306 113 13MB
English Pages [345] Year 1979
Table of contents :
Front Cover
Title Page
Preface
Contents
1 Bonding. The Internal Structure of Solids
§ 1 The van der Waals forces
§ 2 The ionic bond
§ 3 The covalent bond
§ 4 The metallic bond
§ 5 The hydrogen bond
§ 6 Comparison between bonds of various kinds
§ 7 Forces of repulsion
§ 8 Crystal lattice
§ 9 Notation used to describe sites, directions, and planes in a crystal
§ 10 Classification of solids based on the nature of bonds
§ 11 Polymorphism
§ 12 Imperfections and defects of the crystal lattice
2 Mechanical Properties of Solids
§13 Elastic and plastic deformations. Hooke's law
§14 Principal laws governing plastic flow in crystals
§15 Mechanical twinning
§16 Theoretical and real shear strengths of crystals
§17 The dislocation concept. Principal types of dislocations
§18 Forces needed to move dislocations
§ 19 Sources of dislocations. Strengthening of crystals
§20 Brittle strength of solids
§21 Time dependence of fhe strength of solids
§22 Methods of increasing the strength of solids
3 Elements of Physical Statistics
§23 Methods used to describe the state of a macroscopic system
§24 Degenerate and nondegenerate ensembles
§25 The number of states for microscopicparticles
§26 Distribution function for a nondegenerate gas
§27 Distribution function for a degenerate fermion gas
§ 28 Distribution function for a degenerate boson gas
§ 29 Rules for statistical averaging
4 Thermal Properties of Solids
§ 30 Normal modes of a lattice
§ 31 Normal modes spectrum of a lattice
§ 32 Phonons
§ 33 Heat capacity of solids
§ 34 Heat capacity of electron gas
§ 35 Thermal expansion of solids
§ 36 Heat conductivity of solids
5 The Band Theory of Solids
§ 37 Electron energy levels of a free atom
§ 38 Collectivization of electronsin a crystal
§ 39 Energy spectrum of electrons in a crystal
§ 40 Dependence of electron energy on the wave vector
§ 41 Effective mass of the electron
§ 42 Occupation of bands by electrons. Conductors, dielectrics ,and semiconductors
§ 43 Intrinsic semiconductors. The concept of a hole
§ 44 Impurity semiconductors
§ 45 Position of the Fermi level and free carrier concentration in semiconductors
§ 46 Nonequilibrium carriers
6 Electrical Conductivity of Solids
§ 47 Equilibrium state of electron gas in a conductor in the absence of an electric field
§ 48 Electron drift in an electric field
§ 49 Relaxation time and mean free path
§ 50 Specific conductance of a conductor
§51 Electrical conductivity of nondegenerafe and degenerate gases
§ 52 WiedemannFranzLorenz law
§ 53 Temperature dependence of carrier mobility
§ 54 Electrical conductivity of pure metals
§ 55 Electrical conductivity of metal alloys
§ 56 Intrinsic conductivity of semiconductors
§ 57 Impurity (extrinsic) conductivity of semiconductors
§ 58 Deviation from Ohm's law. The effect of a strong field
§ 59 The Gunn effect
§ 60 Photoconductivity of semiconductors
§ 61 Luminescence
§ 62 Fundamentals of superconductivity
7 Magnetic Properties of Solids
§ 63 Magnetic field in magnetic materials
§ 64 Magnetic properties of solids
§ 65 Magnetic properties of atoms
§ 66 Origin of diamagnetism
§ 67 Origin of paramagnetism
§ 68 Origin of ferromagnetism
§ 69 Antiferromagnetism
§ 70 Ferrimagnetism. Ferrites
§71 Magnetic resonance
§ 72 Fundamentals of quantum electronics
8 Contact Phenomena
§ 73 Work function
§ 74 Contact of two metals
§ 75 The metalsemiconductor contact
§ 76 Contact between two semiconductors of different types of conductivity
§ 77 Physical principles of semiconductor pn junction devices
§ 78 Fundamentals of integrated circuit electronics (microelectronics)
9 Thermoelectric and Galvanomagnetic Phenomena
§ 79 The Seebeck effect
§80 The Peltier effect
§81 The Thomson effect
§ 82 Galvanomagnetic phenomena
§ 83 Practical applications of thermoelectric and galvanomagnetic phenomena
Appendices
Appendix I Derivation of the MaxwellBoltzmann distribution function.
Appendix II Derivation of the FermiDirac distribution function.
Appendix III Derivation of the BoseEinstein distribution function.
Appendix IV Tables
Glossary of Symbols and Notations
Bibliography
Index
G. I. Epifanov Mir Publishers Moscow
Solid State Physics
I\ H. EnH(J>aHOB OHsmca TBepjioro Tejia MocKBa, «BLicmaH mKOJia»
Solid State Physics by G. I. Epifanov, D.Sc. Moscow Institute of Electronic Engineering Translated from the Russian by Mark Samokhvalov, Cand. Sc.
Mir Publishers Moscow
Revised from the 1977 Russian edition First published 1979
Ha aneAuucKOM xaune
(O M ii/viT ojibCT D o «BhicmaH niK O Jia*, 1977 CO Helium atoms
Helium atoms
Instantaneous dipoles
Instantaneous dipoles
(a)
(b)
becomes correlated and this leads to the forces of interaction. The forces can be of two types. If the motion of the electrons is correlated, as shown in Figure 1.1(a), the instantaneous dipoles attract each other; if the correlation is as shown in Figure 1.1(b), the resulting interaction is repulsion. Since the realization of the arrangement of Figure 1.1(a) leads to a reduction in the energy of the system, this arrangement is more probable and is realized more frequently. This is in effect the cause of the constantly existing force of attraction between helium atoms. The bonds discussed above that owe their existence to a correla tion in motion of the electrons in adjacent atoms are termed disper sion forces. They were first calculated by F. London in 1930. The calculation was based on the following model: the instantaneous electric dipole of one atom causes the other atom to be polarized and it becomes an induced dipole leading to the realization of the arrangement in Figure 1.1(a), which corresponds to attraction. The calculation had as its final result the following expression for the energy of the dispersion interaction of two particles: tt
3 a 2E exc
U* =  T — ~
(1.2)
Bonding. Infernal Structure of Solids
13
.where a is the polarizability of the particles1, i?exc their energy of excitation, and r the distance between them. Orientational interaction. Should the molecules possess a constant dipole moment Af, that is, should they be polar molecules, an electrostatic interaction would be established between them tending Figure 1.2 Orientational interaction of polar molecules.
0
. 0
0
o o o to arrange the molecules in a strict order (Figure 1.2), since that order corresponds to the minimum energy of the system. The correct orientation of the molecules is disturbed by thermal motion. There fore the energy of the system due to the mutual orientation of the molecules is strongly dependent on temperature. At low tempera tures, when the orientation of the molecules is perfect, the interac tion energy is determined from the expression M2 (1.3) 2jie0r3 where r is the distance between the molecules, and e0the permittivity of free space. In the high temperature range the energy of interaction of polar molecules, as had been demonstrated by W. H. Keesom, is of the following form: M* (1.4) Uor — 24ji26§/cb^^6
The type of interaction discussed above is termed orientational interaction. Induction interaction. Lastly, in case of polar molecules of high polarizability an induced moment due to the action of the field of constant dipoles may be established (Figure 1.3; the induced dipoles are shown by dotted lines). The energy of mutual attraction due to the interaction of the rigid dipole of the first molecule and the induced dipole of the second molecule, as has been shown by Debye, is independent of temperature and is given by the expression am 1 (1.5) 8jtejj r6 1 Let us recall the physical meaning of a. The charges in the molecule are displaced under the action of an external field of intensity %. This leads to a dipole moment M proportional to %: M = a %, the proportionality factor a being the polarizability of the molecule.
14
Solid State Physics
where, as before, M is the constant dipole moment of the molecule^ and a its polarizability. Such interaction is termed induction, or dejormation, interaction. In general, when two molecules are brought close together all three types of interaction may be established, the interaction pnergy being the sum of the energies of the dispersion (t/d), orientational (U0r), and induction (t/ln) types of interaction: U = Ud+ U 0T+ Uin Figure 1.3 Induction interaction of molecules (dotted lines show the induced dipoles).
Table 1.1 shows the relative magnitude (in percent) of each of those components of the total bonding energy for water, ammonia, hydrogen chloride and carbon monoxide. The data presented in Table 1.1 show the induction interaction for all the substances to be weak. Three quarters or a half of the bond energy in substances made up of polar molecules is due to the energy of orientational interaction; while in materials made up of nonpolar molecules almost all of the bond energy is due to the dispersion interaction. Table 1.1 Type of interaction —  : :—:: — : : Dispersion Induction Orientational
Substance Water Ammonia Hydrogen chloride Carbon monoxide
19 50 81 100
4 5 4
77 45 15
Table 1.2 shows the values of the bond energy for some molecular crystals held together by van der Waals forces. Table 1.2 Substance
ub (103 J/mole)
Substance
ub (103 J/mole)
Neon (Ne) Nitrogen (N.2) Oxygen (02)
1.9 6.6 8.2
Argon (Ar) Carbon monoxide (CO) Methane (CH4)
8.4 8.4 10.8
15
Bonding. Internal Structure of Solids
§2 The ionic bond Atoms that occupy places in the Mendeleev periodic table next to inert gases tend to assume the electronic configuration of these gases either by giving away or accepting electrons. The valence electron of alkali metals, which immediately follow the inert gases, moves outside the closed shell and is only weakly connected with the nucleus. The halides, which immediately precede the inert Figure 1.4 Dependence of energy of interacting ions on the distance between them: 1 — energy of attraction, 2 — energy of repulsion, 3 — total energy of interaction.
U
gases, lack one electron to complete a stable shell characteristic of an inert gas. Therefore they exhibit high affinity to an excess elec tron. Such atoms, that is, typical metals and halides, are bonded in the following way. First a recharging of the atoms takes place. The electron from the metal moves over to the halide. This turns the metal atom into a positively charged ion and the haloid atom into a negatively charged one. These ions interact according to the Cou lomb law as two opposite charges. Such a bond became known as an ionic bond. The energy of attraction of two ions separated by the distance r is U a tt
q2
4ne0r
( 1. 6)
where q is the charge of the ions. The curve 1 in Figure 1.4 shows the dependence of C/att on r. As r decreases the absolute value of the energy increases monotonically, tending to infinity as r>0 . The force of attraction tends to bring the ions together as close as possible. This, however, is prevented by the forces of repulsion, which begin to make themselves felt at small distances and rise very rapidly with the decrease in distance. The repulsion energy C/rep is shown in Figure 1.4 by the
Solid State Physics
16
curve 2. Max Born and other scientists expressed the repulsion energy in the form ^rep— rn
(1*7)
where B and n are constants. The resulting interaction energy of two ions is B g rn
(1.8)
Ajieq]
This energy is shown in Figure 1.4 by the curve 3 which has a minimum at r = r0; the depth of this minimum determines the bond energy C/b, and r0 determines the distance between the ions in the molecule. Making use of the fact that in equilibrium (at r = r0) the force of attraction, F att = — (df/att/(ir)r==ro, equals the force of repulsion, F rep = — (dUTev/dr)r = ro, we can easily express (1.8) as
The energy of the lattice made up of N such molecules is
where A is the Madelung constant, which takes account of the energy of interaction of the given molecule with all its neighbouring mole cules in the crystal. Table 1.3 shows by way of an example the experimental values of the bond energy of some ionic crystals and its values calculated with the aid of (1.10). The discrepancies do not exceed 12 percent, which is proof of good agreement between theory and experiment. Table 1.3 w ysia i Sodium chloride (NaCl) Potassium iodine (KI) Rubidium bromide (RbBr) Caesium iodine (Csl)
C/b (103 J/mole) experiment
theory
752 650 635 595
754 630 645 585
§3 The covalent bond The ionic and van der Waals bonds are unable to account for the existence of such compounds as H 2, 0 2, N2, etc., as well as for bonds in atomic crystals of the diamond type. Evidently, atoms of one kind cannot form oppositely charged ions by changing the distribu
Bonding. Infernal Structure of Solids
17
tion of valence electrons, as was the case in the metalhalide interac tion. On the other hand, the bond in the H 2, 0 2, and N2 molecules is much stronger than that which could be attributed to the van der Waals forces. For such compounds the role of the van der Waals forces is that of a small correction to the bond mainly responsible for the strength of the compounds. This bond became known as the covalent bond. Let us consider the nature of this type of bond using the hydrogen molecule as an example. Figure 1.5 Calculating covalent bond between hydrogen atoms: A, B — hydrogen atoms; a, b — their nuclei; 1 — electron of atom A; 2 — electron of atom B ; ral, rb2 — distances of electrons from their nuclei; ri2 — distance between electrons; ra2 — distance of electron 2 from nucleus a; rbl — distance of electron 1 from nucleus b; r — distance between nuclei.
Suppose that two hydrogen atoms are at a rather great distance r from one another. The atom A consists of the nucleus a and the electron 1 and the atom B consists of the nucleus b and the electron 2 (Figure 1.5). Since the density of the electron cloud which describes the electron state in an atom falls off very rapidly as the distance from the nucleus increases, the probabilities to discover electron 1 near nucleus b and electron 2 near nucleus a are very small. Calcula tion shows that for r ^ 50 A each electron can visit the other nucleus on the average only once in 1012 years. Because of that atoms A and B may be regarded as isolated atoms and the energy of the system made up of such atoms may be taken to be equal to 22?0, where F 0 is the energy of the isolated atom in the ground state. When the atoms are brought closer together, the probability of the electrons going over to nuclei other than their own increases. For r « 2 A the electron clouds begin to overlap noticeably and the transition frequency rises up to 1014 s “ l. If the atoms are brought still1closer together, the frequency of the electron exchange rises so that it becomes meaningless to speak of electron 1 as belonging to the atom A and of electron 2 as belonging to atom B. This corres1!—0885
18
Solid State Physics
ponds to a new state that is not characteristic for a system made up of two isolated atoms. A remarkable property of this new state is that the electrons in it belong simultaneously to both nuclei, in other words, aje collectivized. The collectivization of the electrons is accompanied by a change in electron density distribution  i; 2 and in the energy of the system as compared to the total energy 2E 0 of the isolated atoms. The dotted lines 1 in Figure 1.6 show the electron cloud density of the isolated atoms, the thin solid line 2 shows the total density obtained by simple superposition of the electron clouds of isolated atoms, and the thick Figure 1.6 Electron density distribution in a system of two hydrogen atoms: 1 — electron density distribution in isolated hydrogen atoms, 2 — electron density resulting from simple overlapping of electron clouds of isolated atoms brought together to within a distance of r, 3 — actual electron density distribution in a hydrogen molecule.
solid line 3 the actual density distribution along the axis joining the nuclei a and b brought about by the collectivization of the electrons. The figure shows that the collectivization of the electrons results in the electron clouds being drawn into the space between the two nuclei: at a small distance from the nucleus outside this space the density of the clouds falls off, as compared with the density in isolated atoms, at the same time rising in the space between the nuclei above the sum of the densities of isolated atoms. The appear ance of a state with an electron cloud of increased density that fills the space between the nuclei always results in a decrease in the system ’ s energy and in the appearance of forces of attraction between the atoms. Speaking figuratively, we may say that the electron cloud formed in the space between the nuclei by a collectivized pair of electrons draws the nuclei together, striving to bring them as close together as possible. Such is the qualitative picture of the origin of the covalent bond. Quantitative calculations of the hydrogen molecule were first
Bonding. Internal Structure of Solids
19
performed by W. H. Iieitler and F. London in 1927. Those calcula tions have shown that a system consisting of two closely spaced atoms of hydrogen can have two energy values depending on the direction of the electron spins in the atoms: Us = 2E0+ £ ± £
(1.11)
when the spins are antip^arallel, and Ua = 2E0+ ^ £
(1.12)
when the spins are parallel. Here 2E 0 is the total energy of the two isolated atoms, K is the energy of the electrostatic interaction of the electrons with the nuclei, of the electrons with one another, and of the nuclei. Another name for it is Coulomb energy. Its sign is nega tive. By A we denote the energy of exchange interaction due to the atoms exchanging electrons. This is the additional energy that ap pears as the result of the change in the electron density distribution in the process of the formation of the molecule. Its sign is negative and its absolute value is much larger than K ( A  >  K ); 5 is the overlap integral whose value lies within the limits 0 ^ S ^ 1. The state with the energy Us is termed symmetric and with Ua antisymmetric. Since both K and A are negative and 5 ^ 1 , the energy of the system in the symmetric state is less than the energy of two isolated atoms U5 < 2 E 0 (1.13) This corresponds to the appearance of forces of attraction. Since the absolute value of the exchange energy A is considerably greater than that of the Coulomb energy K the decrease in the system ’ s energy is mainly due to A. For this reason the force of attraction that appears between the atoms is termed the exchange force. For the same reason, that is, because  A   K , the formation of the antisymmetric state leads to an increase in the system ’ s ener gy. This corresponds to the appearance of repulsive forces. Figure 1.7 shows the dependence of Us and t/a on r/a, where r is the distance between the atoms, and a = 0.529 A is the radius of the first Bohr orbit (the Bohr radius). The zeroth energy level has been fixed at 2E 0. Figure 1.7 shows that in the antisymmetric state the system ’ s energy rises steadily as the atoms are brought closer together (curve 7), this corresponding to the mutual repulsion of the atoms. Therefore a hydrogen molecule cannot be formed in such a state. In the symmetric state (curve 2) the system ’ s energy at first falls as the distance r between the atoms decreases, attaining its minimum value at r = r0. As the distance r decreases still further, the energy begins to rise because of the appearance of strong repulsive
20
Solid State Physics
forces. The existence of a minimum on the potential energy curve makes the existence of a stable system of two hydrogen atoms, that is, a hydrogen molecule, possible. To destroy this system work must be performed equal to the depth of the potential well, Uh. Calculation provides the following values of t/b and r0: Z7b = = 4.37 eV, r0 = 0.735 A; the experimental values are C/b = = 4.38 eV, r0 = 0.753 A. The agreement between theory and ex periment is quite good. Table 1.4 shows the values of the bond energy for some covalent compounds—the molecules of H 2, N2, 0 2, CO—and for diamond, silicon and germanium crystals in which the bonding is due to covalent forces. Figure 1.7 Interaction energy of two hydrogen atoms: 1 — antisymmetric state, 2 — symmetric state.
The data show the covalent bond to be a very powerful one, its energy being as high as 10ft106 J/mole. Table 1.4 Gas
u \> (10B J/mole)
Crystal
Ub (106 J/mole)
Carbon monoxide (CO) Nitrogen (N2) Oxygen (0?) Hydrogen (H2)
10.8 9.5 5.0 4.4
Diamond (C) Silicon (Si) Germanium (Ge)
6.8 4.4 3.5
Characteristic properties of the covalent bond, which distinguish it] from the bonds of other types, are its saturability and direc tionality. Saturability means that each atom can form covalent bonds only with a limited number of its neighbours. This means that each hydrogen atom can form covalent bonds only with one of its neigh bours. The electron pair constituting such a bond has antiparallel
21
Bonding. Infernal Structure of Solids
spins and occupies one quantum cell. A third atom in this case instead of being attracted will be repelled. The valence bond is formed in the direction of the greatest density of the electron cloud corresponding to the valence electrons. In this case there is maximum overlapping of the electron clouds of the bonding electrons, which implies that the valence bond is directional.
§4 The metallic bond There is a special group of substances, called metals, that occupy places at the beginning of every period of the Mendeleev table. The formation of the metallic bond cannot be explained by the presence of the ionic or the covalent bond. Indeed, the ionic bond Figure 1.8 Electron density distribution in the aluminium lattice obtained by Xray photography.
appears only between atoms having different affinities to the addi tional electron, for instance, between the atoms of a metal and a halide. Evidently, such bond between kindred atoms of a metal having identical affinity to the electron is impossible. On the other hand, metallic atoms do not have enough valence electrons to form valence bonds with their nearest neighbours. For instance, the copper atom has one valence electron and can form a valence bond only with a single atom. But in the copper lattice every atom is surround ed by twelve neighbours with which it must be connected by lines of force. This points to the fact that in metals there is a special type of bonding known as the metallic bond. Let us consider the nature of this bond. In metallic atoms the external valence electrons are rather weakly coupled to the nucleus. In the liquid and solid states the atoms come so close together that the valence electrons are able to leave their respective atoms and wander throughout the lattice. This leads to an extremely homogeneous distribution of the negative charge in the crystal lattice. This conclusion is supported by direct experiments. Figure 1.8 shows an experimental curve of the electron density
22
Solid State Physics
distribution between the sites of the aluminium lattice obtained by means of Xray photography. Most part of the distance between the sites the electron concentration remains constant. Only quite close to the sites it rises sharply because of the presence of internal shells of the aluminium atoms. In the lattice of a metal the bond is due to the interaction of the positive ions with the electron gas. The electrons moving between the ions compensate the forces of repulsion existing between the positively charged ions and draw them closer together. As the distance between the ions becomes smaller the density of the electron gas rises and this leads to an increase in the force drawing the ions to gether. On the other hand, in this case the repulsive forces acting between the ions tend to move them away from each other. When the distance between the ions becomes such that the forces of attrac tion are compensated by the forces of repulsion, a stable lattice is formed. It appears that the metallic bond is somewhat similar to the valence bond, since they are both based on the collectivization of external valence electrons. However, in case of the valence bond only atoms that form pairs of nearest neighbours take part in the collectivization of electrons, and the respective electrons always remain between the atoms. In case of the metallic bond all atoms of the crystal take part in the collectivization of electrons, and the collectivized electrons are no longer localized near their respective atoms but move freely inside the lattice.
§5 The hydrogen bond The hydrogen bond is formed between an atom of hydrqgen and an extremely electronegative atom, for instance, an atom of oxygen, fluorine, nitrogen, chlorine. Such an atom attracts the bonding electrons and becomes negatively charged; the hydrogen atom after losing the bonding electron assumes a positive charge. The hydrogen bond is a result of electrostatic attraction of those charges. As a typical example we may cite the hydrogen bond between molecules of water (Figure 1.9). The 0 —H bond between an oxygen atom of one molecule and a hydrogen atom of another behaves as a tiny dipole with a —8 charge on the oxygen atom and a +8 charge on the hydrogen atom. The force of attraction between those charges is the cause of the hydrogen bond shown by dots in Figure 1.9. The attraction is enhanced by the small dimensions of the hydrogen atom that enable it to come close to the electronegative atom. Still, this distance r0n = 2.76 A is much greater than the radius of the covalent bond H —0, r0, in the water molecule itself, which is equal to 0.96 A. This is quite natural since the energy of the covalent
23
Bonding. Internal Structure of Solids
bond is about an order of magnitude higher than that of the hydrogen bond. Its value for water is (2125) X 10* J/mole. The hydrogen bond is the cause of association of molecules of liquids (water, acids, spirits, etc.), which results in greater viscosity, higher boiling point, abnormal thermal expansion, etc. Water may serve best to illustrate this. Should there be no hydrogen bonds between the molecules of water, its boiling point at atmospheric Figure 1.9 Hydrogen bond between water molecules.
H'
pressure would be not f100 °C but —80 °C and its viscosity would be lower by almost an order of magnitude. When water is heated above 0 °C, the hydrogen bond is destroyed. Since the hydrogen bond is responsible for the loose structure of associated complexes, in which the water molecules are rather far apart (2.76 A), the destruction of such a loose structure should result in an increase in the density of water. On the other hand, an increase in the temper ature of water and a corresponding increase in the intensity of thermal motion of its molecules should lead to thermal expansion and a decrease in its density. Experiment shows that in the tempera ture range 04 °C the first factor—the increase in density due to the disruption of the hydrogen bonds—is the prevalent one. Because of that within this range the density of water rises upon heating. Above 4 °C the other factor—thermal expansion—prevails. This is why when water is heated above 4 °C its density decreases, as is the case with other (normal) liquids.
§6 Comparison between bonds of various kinds The van der Waals bond is the most universal one. It exists in all cases without exception. At the same time this is the weakest, having an energy of the order of 104 J/mole. Ideally, it operates between neutral atoms, or molecules, with closed inner electron shells. Specifically, the van der Waals forces are responsible for the
24
Solid State Physics
existence of the liquid and solid states of inert gases, hydrogen, oxygen, nitrogen and many other organic and inorganic compounds. They also, as we will see later, form bonds in many of the molecular valence crystals. Because of low energy values of the van der Waals bond all structures based on it are unstable, volatile and have low melting points. The ionic bond is a typical chemical bond very * frequent among the inorganic compounds such as metalhalide compounds, metallic oxides, sulfides and other polar compounds. The ionic bond is also a feature of numerous intermetallic compounds (carbides, nitrides, selenides, etc.). The energy of the ionic bond is much higher than that of the van der Waals bond and may be as high as 10° 3/mole. Because of that solids based on the ionic bond have high sublima tion heat values and high melting points. The covalent bond is extremely widespread among organic com pounds, but is also present in inorganic compounds, in some metals and in numerous intermetallic compounds. This bond is responsible for the existence of valence crystals of the diamond, germanium and other types, as will be discussed below. The energy of the covalent bond is also high ( ^ lO 15 J/mole), which stems from the fact that the solids with this type of bond have high melting points and high heats of sublimation. The metallic bond formed as a result of the collectivization of the valence electrons is characteristic of typical metals and numerous intermetallic compounds. The order of magnitude of the energy of this type of bond is comparable to that of the energy of covalent bond. Lastly, the hydrogen bond, although relatively weak, still plays an important part in nature. It should be pointed out that in real solids no types of bonds discussed above ever exist purely by themselves. Practically, there is always a superposition of two types of bonds or more. One of them, as a rule, plays a dominant part in determining the structure and the properties of the solid.
§7 Forces of repulsion For the formation of a stable system of interacting atoms or mole cules, together with forces of attraction there should be forces of re pulsion, which would prevent the complete merging of the particles. The origin of the forces of repulsion is first of all the interaction of the nuclei each of which carries a considerable positive charge. The energy of this interaction, £^ep> depends on the distance be tween the nuclei and on the degree of screening by their internal electron shells.
Bonding. Internal Structure of Solids
25
The following expression for Urep may be obtained from quantum mechanical calculations: ff«pOCe“r/a (i14) where r is the distance between the nuclei, and a = 0.529 A the Bohr radius. This dependence of t/^ep on r determines the nature of the forces of repulsion: they attain enormous values at short distances and fall off abruptly as r increases. For instance, when the distance between a proton and a hydrogen atom decreases from r = 2a to r = a!2 (4 times), the repulsive energy increases almost 300fold. The repulsive forces due to the interaction of the nuclei play a dominant role when light atoms, whose nuclei are rather poorly screened by the electron shells, are brought together. In all other cases the dominant part is played by repulsion due to the overlapping of closed electron shells of the atoms being brought together. Consid er by way of an example the interaction between a chlorine ion with a closed 3p shell and a sodium ion with a closed 2p shell. When the ions are brought together to a distance at which the 3p and 2p shells overlap, the number of electrons in each of them begins to exceed that which is compatible with the Pauli exclusion principle. Because of that some of the electrons are forced to go to higher energy levels (for instance, 3d or 4s). This results in an increase in the system ’ s energy and, consequently, in the appearance of forces of repulsion. Quantum mechanical calculations show the energy of such repulsion to have an exponential dependence on the distance, as well:
Uf;9pOCe'/e
(1.15)
where p is a constant usually obtained experimentally. Often the repulsion energy is expressed in the form (1.7). This expression gives a less steep decline of C/rep with the increase in r and is less consistent with experiment than (1.14) or (1.15) but is nevertheless widely used by researchers.
§8 Crystal lattice No matter what the origin of forces appearing when particles are brought together is, their general nature is the same (Figure 1.10(a)): at comparatively large distances forces of attraction F att increase rapidly as the distance between the particles decreases (curve 1); at small distances forces of repulsion Fre^ come into being and with a further decrease in r they increase much more rapidly than Fatt (curve 2). At the distance r = r0 the repulsive forces counterbalance the forces of attraction, the resultant force ofAinteraction F vanishes
26
Solid State Physics
Figure 1.10 Interaction between approaching particles: (a) — interaction forces, 1 — force of attraction, 2 — repulsive force, 3 — resultant force; (b) — interaction energy.
(curve 5), and the energy attains its minimum value Uh (Fig ure 1.10(b)). Because of this the particles brought together to a distance r0 are in a state of stable equilibrium. By the same reason the free particles should arrange themselves in a strict order at a distance r0 from one another thus forming a b o d y . with a regular internal struc ture—a crystal. Such a structure will remain stable until the abso lute value of the bond energy remains greater than the energy of thermal motion of the parti cles. The particles constituting the crystal cannot freeely leave (b) their equilibrium sites because this involves an increase in their energy and leads to the appearance of forces tending to return them to their equilibrium sites. One may say that the particles are fixed in their equilibrium sites. The only form of motion allowed to them are random vibrations around their equilibrium sites. To describe the regular internal structure of crystals one may conve niently use the concept of the crystal lattice. There are lattices of two types — the translational Bravais lattice and the lattice with a basis. Bravais lattice. From the geometrical point of view a regular periodic arrangement of particles may be described with the aid of a translation. Figure 1.11(a) shows a lattice obtained with the aid of translation of a particle along the three axes: OX over the sec tions a, 2a, 3a, . . ., ma, . . .; OY over the sections b, 2ft, 3b, . . . . . ., nb, . . .; OZ over the sections c, 2c, 3c, . . ., pc, . . . (m, n, p are integers). The position of any particle in this lattice is described by the vector r = ma rib + pc (1.16)
Bonding. Infernal Structure of Solids
27
The vectors a, b, c are termed the translation vectors and their nume rical values the translation periods. A lattice built with the aid of translation of any site along the three directions is termed a Bravais lattice. The smallest parallelepi ped built on the vectors a, b, c is termed the unit cell of the crystal (Figure 1.11(b)). The shape and the volume of all the unit cells Figure 1.11 Crystal lattice: (a) — Bravais lattice, (b) — unit cell of Bravais lattice.
comprising the lattice are identical. All cell apexes are occupied by identical atoms or groups of atoms and are therefore equivalent. They are termed lattice sites. To discribe a unit cell, six quantities should generally be stated: three edges of the cell (a, 6, c) and three angles between them (a, P, y). Those quantities are termed the parameters of the unit cell. Often the sections a, b, c are used as units of length in lattices instead of the metre. They are termed axial units. Unit cells with particles only at the vertices are known as primi tive cells. There is only one particle to each such cell. In some cases to express the lattice symmetry more fully the unit cells are built so that they contain particles not only in their apexes but at other points as well. Such cells are termed complex cells. The most widespread types of such cells are (Figure 1.12) the bodycentered (BC), the facecentered (FC), and the basecentered (BaseC) cells. It may be shown that such cells may easily be reduced to prim itive cells. Because of that they are Bravaistype cells. A lattice with a basis. Not every type of lattice may be obtained by translation of a single site. Figure 1.13 shows a twodimensional lattice with a generaltype basis. It may easily be seen that it is impossible to describe the unit cell of such a lattice in terms of
Solid State Physics
28
a singlesite unit cell. Such a lattice may be imagined as consisting of two Bravais lattices, 1 and 2, each determined by the basis vec tors a and b and inserted into each other. The relative displacement of the lattices is described by an additional basis vector A. The number of such basis vectors may be arbitrary. /r
Figure 1.12 Typical crystal structures: (a) — basecentered (BaseC); (b) — bodycentered (BC); (c) — facecentered (FC).
The lattice of this type is termed the lattice with a basis. It may be built with the aid of the same translations as can be used to build. any of the Bravais lattices that make it up. However, in this case we shall have to translate not one site but several sites—the basis,

4


4
i i •—i
0
b! i [o'
9 9
>
b
Figure 1.13 Twodimensional lattice with a basis: A — basis vector.
1 — 1 — " 1 1
’
o1 1 1
Sublattice 1 Sublattice 2
 6
defined by the totality of the basis vectors. Thus, the twodimen sional lattice shown in Figure 1.13 may be obtained by a translation of the basis made up of two sites: 0 and O'. An example of a threedimensional lattice with a basis is the diamond lattice shown in Figure 1.14(a). It m aybe obtained by inserting one FCC (facecentered cubic) lattice into another FCC lattice displaced along the space diagonal by onefourth of its length. Figure 1.14(h) shows a tetra hedron designated by a dotted line in Figure 1.14(a). It may be
29
Bonding. Internal Structure of Solids
Figure 1.14 Diamond lattice: (a) — spatial arrangement of atoms in the lattice; (b) tetrahedral pattern of atoms in the lattice.
seen from Figure 1.14(b) that in the diamond lattice every atom is surrounded by four nearest neighbours in the apexes of the tetra hedron whose edge is a/2.
§9 Notation used to describe sites, directions, and planes in a crystal Let us mention briefly the notation conventionally used to describe sites, directions and planes in a lattice, the Miller indices. Site indices. The position of any lattice site relative to the chosen origin of coordinates is defined by three of its coordinates (Figure
Z
Figure 1.15 Indices of a crystal lattice site.
1.15): x, y, z. These coordinates may be expressed in the following form: x = ma, y = nb, z = pc where a, 6, c are the lattice parameters, and m, n, p are integers.
30
Solid State Physics
Should we use lattice parameters as units of length along the respective axes we would obtain the lattice coordinates simply in the form of numbers m, n, p. These numbers are termed site indices and are written in the form [[mnp]]. For a negative index the minus sign is written above the index. For instance, for a site with coordi nates x_= —2a, y = — lb, z = 3c the indices are written in the form [213]. Indices of direction. To describe a direction in a crystal a straight line passing through the origin is chosen. The position of this is uniquely defined by the indices of the first site through which it passes (Figure 1.15). Therefore the indices of the site are at the same time the indices of the direction. The usual notation for a di rection is [mnp]. The indices of direction are, by definition, the three smallest integers that describe the position of the site nearest to the origin which lies on the given direction. For instance, the indices of the direction that passes through the origin and the site [[435]] are [435]. Figure 1.16 shows the principal directions (crystal lographic orientations) in a cubic crystal and their notation. Plane indices. The position of a plane is defined by the choice of three sections A, B, C it cuts off when it intersects with the three coordinate axes. The procedure of finding the indices of such a plane is as follows. The sections ABC are expressed in axial units and the reciprocal quantities are written as 11A, 1IB, IIC. A common denominator is found for all the three fractions. Suppose it is D. Then the integers h = DIA, k = D IB, I = DIC will be the plane indices. They are written in the form (hkl). Determine, for example, the indices of a plane that cuts off the sections A = 1/2, B = 2, C = 1/3 on the X, Y , Z axes respectively. The ratios 1/A f 1IB  l/C = l/(l/2)  1/2  l/(l/3) = 2 1/2 f 3. The common denominator is D = 2. The indices of the plane are h = 2/(l/2) = 4, k = 2/2 = 1, I = 3/(l/2) = 6. The plane is denoted (416). Figure 1.17 shows the principal planes of the cubic lattice. It may easily be shown that in a cubic crystal the distances be tween the planes belonging to a given family may be expressed with the aid of the indices of these planes in the following way: y&2+fc2+z2 ' where a is the lattice parameter. This formula shows that the greater are the plane indices the shorter is the distance between the planes. To denote the planes in a hexagonal crystal a fouraxis coordinate system is used (Figure 1.18): three axes (ax, a2, a3) make angles of 120° with one another and lie in the base of a hexagonal prism, the fourth axis, c, being perpendicular to the base plane. Every
Bonding. Internal Structure of Solids
Figure 1.16 Indices of principal directions in a cubic crystal.
Figure 1.17 Indices of principal planes in a cubic crystal.
31
32
Solid State Physics
plane is denoted by four indices: hkil. The additional label i occupies the third place and is calculated with the aid of h and k: i\= = — (h + k). The base plane parallel to the axes au a2, a3 has Figure 1.18 Indices of principal planes in a hexagonal crystal.
the indices (0001). The planes parallel to the lateral faces of the prism have indices of the (1010) type. There are three such planes (not parallel to one another). They are termed firstorder planes.
§10 Classification of solids based on the nature of bonds The nature of the crystal structure is primarily dictated by the nature of bonding forces acting between the structural particles (atoms, ions, molecules) which make up the solid. In accordance with the five existing types of bonds there are five principal types of crystal lattices: ionic, or coordination, lattices, with the ionic bond playing the main part; molecular lattices, with the van der Waals forces mainly responsible for the bonding; atomic lattices, with bonds of a distinctly covalent type; metallic lattices, with characteristic metallic bonds; and lattices with the hydrogen bond. Let us analyze from this viewpoint the crystal structure of chemi cal elements and of typical chemical compounds (see Appendix IV, Table 1). The chemical elements may be roughly divided into four classes according to the type of crystal structure. The analysis may best be started with Class IV. Class IV. This class includes all the inert gases. In the process of compression and crystallization of these gases only comparatively weak van der Waals forces act between the atoms, which have spher ically symmetrical electron shells. Acted upon by these forces the symmetrical atoms draw together to form a most tightly packed
33
Bonding. Internal Structure of Solids
facecentered cubic lattice. Every atom is surrounded by 12 nearest neighbours. The number of nearest neighbours is usually termed the coordination number of the lattice. Class III. The Class III includes silicon and carbon from the short periods of the Mendeleev periodic table, germanium and tin from Group IVB, and all the elements from Groups VB, VIB, VIIB. Figure 1.19 Crystal structure of shemical elements crystallizing in accordance with the (8—N)rule: (a) — elements of Group IVB; (b) — elements of Group VB; (c) — elements of Group VIB, (d) — elements of Group VIIB.
(a)
(b)
(c)
(d)
The crystallization of the elements of those classes proceeds in con formity with the (8 — V)rule: every atom in the lattice is surround ed by 8 — N nearest neighbours, N being the number of the group to which the element belongs. Thus diamond, silicon, germanium and gray tin are elements of Group IV of the Periodic Table. There fore the coordination number of their lattices should be 8 — 4 = 4. They all do have a tetrahedral lattice in which every atom is sur rounded by 4 nearest neighbours, as is shown in Figure 1.19 (a). Phosphorus, arsenic, antimony and bismuth belong to Groug V. Their coordination number is 8 — 5 = 3. Every atom has 3 nearest neighbours lying in a plane, as shown in Figure 1.19(b). Their lattice has a laminate structure, with the atomic layers bonded by van der Waals forces. Selenium and tellurium belong to Group VI and have a coordina tion number 2. Their atoms form long spiralshaped chains with each atom having two nearest neighbours (Figure 1.19(c)). The chains are bonded by van der Waals forces. Lastly, iodine belongs to Group VII (Figure 1.19(d)) and has a coordination number 1. The atoms in the iodine lattice are arranged in pairs bonded by van der Waals forces. This explains the high volatility of iodine.
Solid State Physics
34
Such nature of the crystal structure of chemical elements whose crystallization conforms to the (8— AQrule is quite understandable. The atoms of Group IV elements have 4 electrons in their outer shell. They lack 4 additional electrons to make up a stable 8electron configuration. They make up the deficit by exchanging electrons with 4 nearest neighbours, as shown in Figure 1.19(a), forming a strong covalent bond with each of them. Accordingly, every atom in the crystal lattice of those elements has 4 nearest neighbours. In the same way the electron shells of Groups V, VI, VII are complet ed to contain 8 electrons. * Many chemical compounds crystallize in crystals with covalent bonds. Quartz Si0 2 may serve as a typical example. In the quartz Figure 1.20
Structure of quartz Si02 crystal.
crystal every silicon atom is surrounded by a tetrahedron of oxygen atoms (Figure 1.20) bonded to the silicon atom by covalent bonds. Every oxygen atom is bonded to two silicon atoms thereby joining two tetrahedrons. In this way a threedimensional net of Si—0 —Si bonds is formed, and the hardness and the melting point of the resulting crystal are high. It may be of interest to note that the Si—0 —Si bonds may be arranged into a onedimensional chain. Such compounds described by the common formula R R R I I I ... _ 0 — Si — 0 — Si — O  S i  O  ... I I I R R R , '
n where R is an arbitrary organic group, are termed silicones. The number n in a chain may be as high as several million. The chains may be joined together with the aid of the lateral groups R. In this way new materials, silicone resins, are formed. Because of the high strength of the Si—0 —Si bonds and of the high flexibility of silicone
Bonding. Internal Structure of Solids
36
chains such resins retain their properties at much lower and much higher temperatures than natural rubbers. This fact enables them to be used for thermal shielding of space ships and aircraft, as well as in extreme arctic conditions. Class I. This is the most populated class which contains metals. Since metallic lattices are made up not of atoms but of ions, having the spherical symmetry of the atoms of inert gases, it is to be expected that metals too should crystallize into the same tightly packed lattices as the inert gases. Indeed, the following three types of crystal lattices are characteristic for metals: the facecentered cubic lattice with the coordination number 12 (see Figure 1.12), the hexagonal closepacked (HCP) lattice with the coordination number 12 (see Figure 1.18) and the bodycentered cubic lattice with the coordination number 8 (see Figure 1.12). The latter is the least closely packed metal lattice. Class II. The chemical elements belonging to Class II are in a sense intermediate between metals and the Class III elements, which crystallize in conformity with the (8 — JV)rule. For instance, the Group IIB elements Zn, Cd and Hg are metals and one would expect them to have a typically metallic lattice with a high coordination number. Actually, Zn and Cd crystals are a special modification of the compact hexagonal lattice in which every atom has 6 nearest neighbours instead of 12, as required by the (8 — A)rule. These atoms occupy the base plane. In the case of mercury the (8 — Ar)rule is observed even more strictly: its crystal structure is a simple rhombohedral in which every atom is surrounded by 6 nearest neighbours. Boron—an element of Group IIIB —has a lattice that may be described as a deformed lattice with 5 nearest neighbours. This too agrees with the (8 — 7V)rule. The ionic bond, as was stated above, plays one of the main parts in the world of inorganic compounds, in particular, in numerous ionic crystals typically represented by the rock salt crystal NaGl (Figure 1.21). In such crystals it is impossible to pick out single molecules. The crystal should be regarded as a closely packed system of positive and negative ions whose positions alternate so that the electrostatic attraction between the nearest neighbours wTould be at its maximum. With the most favourable relation between the radii of the positive {M+) and the negative (X") ions which exists in the NaCl crystal the ions “ touch”one another (Figure 1.22(a)) and the closest possible packing is achieved, in which every ion is surrounded by 6 nearest neighbours of the opposite charge. When the ratio of the radii of the ions M +and is less favourable (Figures 1.22(b, c)) crys tal structures with other coordination numbers, 4 or 8, are formed. Ionic compounds of the M X 2 type, such as CaCl2 and Na20, have still more complex lattices. But the principle upon which they are built remains the same: the ions are packed so as to be surrounded
36
Solid State Physics
by ions of the opposite sign in accordance with the formula of the compound and the ratio of their radii. Finally, let us consider crystals featuring the hydrogen bond. A typical representative of such crystals is ice. Figure 1.23(a) shows a twodimensional diagram of the arrangement of water molecules in an ice crystal: each molecule is surrounded by four nearest neigh bours a distance r0h = 2.76 A away from it with whom it forms hydrogen bonds. In space the molecules occupy the vertices of a Figure 1.21 Structure of rock salt NaCl crystal.
regular tetrahedron (Figure 1.23(b)). The combination of such tetrahedra forms the regular crystal structure of ice (Figure 1.23(c)). The structure is very loose and this is the cause of the abnormally low density of ice. Upon melting, some ( ~15 percent) of the hydro gen bonds are disrupted and the packing density of the water mole cules rises somewhat with the resultant rise in the density of water: the density of ice at 0 °G is 916.8 kg/m3, and the density of water at this temperature is 999.87 kg/m3. It may be of interest to note that if there was no hydrogen bond the melting point of ice would be —100 °C instead of 0 °C. It should finally be stressed again that the hydrogen bond plays an extremely important part in vital biological compounds: protein molecules owe their helical shape exclusively to the hydrogen bond; the same type of bonds holds together the double helixes in the DNA. “It is no exaggeration to claim that life on our planet would have assumed radically different forms—if any at all—were hydrogen bonding not present in water and in the proteins and nucleic acids that compose living cells and that transmit hereditary traits.” 2 2 G. C. Pimentel and R. D. Spratley, Chemical Bonding Clarified Through Quantum Mechanics, HoldenDay, San Francisco (1969), p. 261
37
Bonding. Internal Structure of Solids
Figure 1.22 Effect of relative dimensions of ions on their[ packing in the lattice.
(a)
o  M + (b'
•x
(c)
(d)
Figure 1.23 Crystals with hydrogen bond: (a) — plane diagram of arrangement of water molecules in an ice crystal; (b) — spatial arrangement of water molecules in an ice crystal; (c) — crystal structure of ice,
38
Solid State Physics
Table 2 of Appendix IV shows the general classification of solids. The upper left corner contains typical metals with collectivized electrons (silver, copper) and the upper right corner typical valence crystals with distinctly localized electron bonds. The extreme righthand part contains crystals with van der Waals bonds. Such elements as silicon and germanium occupy an intermediate position between the metals and the valence crystals. At absolute zero they are typical valence crystals; however, as temperature rises the valence bond is gradually disrupted and they begin to exhibit metallic properties. Such solids as sulphur, phosphorus, and selenium occupy an inter mediate position between the valence crystals and crystals with the van der Waals bond. The lower left corner of the diagram contains alloys of the NiCu type with the characteristic metallic bond and the lower right corner —ionic crystals (sodium chloride). Intermediate positions between them are occupied by numerous intermetallic compounds of the Mg3Sb2 type featuring the ionic bond (Mg3Sb2 corresponds to a a Mg+2Sb~3 compound). Intermediate position between the ionic and the valence crystals is occupied by such compounds as S i0 2 and SiC, with bonds of partially ionic nature made possible because of electron displacement. Compounds of the FeS and the T i0 2 (tita nium dioxide) type occupy an intermediate position between ionic crystals and crystals with the van der Waals bond. There’ are a great many crystals in which ionic or covalent bonds act in atomic planes while the bonds between the planes are of the van der Waals type.
§11 Polymorphism Some solids have two or more crystal structures each of which is stable in an appropriate range of temperatures and pressures. Such structures are termed polymorphic modifications, or polymorphs, and the transition from one modification to another, polymorphic transformation. It is the practice to denote polymorphic modifications by Greek letters: the modification stable at normal and lower temperatures is denoted by a; modifications stable at higher temperatures are denoted by the letters p, y, 6, etc. The polymorphism of tin may serve as a classical example. Below 13.3 °C the stable modification of tin is aSn, which has a tetragonal cubic lattice of the diamond type. This is the socalled gray tin. It is brittle and may easily be ground to powder. Above 13.3 °C aSn transforms into pSn, which has a bodycentered tetragonal lattice. This is the familiar white metallic tin, a rather ductile metal. The transformation from p~Sn to aSn is accompanied by a considerable increase in specific volume
Bonding, internal Structure of Solids
39
(by about 25 percent). Long ago when many things were made of tin, the perplexing phenomenon of growing bulges on them and their subsequent destruction following excessive cooling was attri buted to a mysterious metal disease, the “ tin plague”. Many other chemical elements also exhibit polymorphism: carbon, iron, nickel, cobalt, tungsten, titanium, boron, berillium, and others, as well as many chemical compounds and alloys. An interesting and a practically important case of polymorphism is that of carbon, which exists in the forms of diamond and graphite. Figure 1.24 Crystal structure of graphite.
This case deserves a more detailed study. In the diamond lattice every atom is surrounded by 4 nearest neighbours occupying the vertices of a tetrahedron (see Figure 1.14) with whom it is bonded by strong covalent forces. The length of the bond is 1.544 A and the energy per bond is about 3.5 X 105 J/mole. The graphite lattice is of the pattern characteristic of the Group VB element lattices: the carbon atoms form twodimensional layers in which every atom is surrounded by 3 nearest neighbours with whom it is bonded by covalent bonds (Figure 1.24). The length of the bond is r01 = 1.42 A, that is, less than in the diamond lattice, therefore the former is stronger. The distance between the layers is much greater than the length of the C—C bond, being equal to r02 = 3.6 A. Only weak van der Waals forces can act at such great distances and the layers are held together by them. The energy of this bond is (48) X 103 J/mole. Such a great difference in the nature of the bonding forces in the diamond and graphite structures should evidently manifest itself in a great difference in their properties, which is actually the case.
40
Solid State Physics
Diamond is extremely hard and strong and is an ideal abrasive. Graphite slides easily along the planes held together by weak van der Waals forces. Therefore it is used to advantage in making “ lead” pencils and as dry lubricant. The electrons in diamond are held securely between the atoms forming bonds. Light of the visible part of the spectrum is unable to knock out such electrons and there fore is not absorbed in diamond. Because of this diamond is an ideal transparent crystal unable to conduct electric current (a dielectric). In graphite one of the four valence electrons of the carbon atom is actually collectivized by the atoms forming the layer. Such elec trons can easily be moved by the action of an external electric field, making graphite a twodimensional conductor. The presence of mobile electrons explains light absorption (the gray colour of graphite) and its characteristic metallic glitter. In normal conditions graphite is a somewhat more stable modifi cation than diamond, although the difference in the energies of those modifications is quite sm all— of the order of 2 x 103 J/mole: C (diamond)> C (graphite). At/ = —1.88 X 103 J/mole Still, such a difference is enough to bring about a sufficiently rapid transformation of diamond into graphite when heated above 1000 °C in the absence of air. The density of diamond is greater than that of graphite (3500 and 2250 kg/m3 respectively), which is due to a loose packing of the atomic layers in graphite. Therefore at greater pressures diamond becomes more stable and graphite less stable. At sufficiently high pressures diamond becomes more stable than graphite. In such condi tions by raising the temperature to increase the m obility of the carbon atoms we may bring about the transformation of graphite into diamond. The conditions for such transformation to proceed at a practical rate were calculated by the Soviet physicist O. I. Leipunskii. He writes: “ Firstly, graphite should be heated to at least 2000 °C for the carbon atoms to be able to move from place to place. Secondly, it must be subjected to very high pressure, not less than 60 000 at m ospheres.” 3 These conditions were first achieved by the scientists of the General Electric Research and Development Center, who in 1954 succeeded in producing the first synthetic diamonds in the form of dark unsightly crystals, the largest being 1.5 mm long. Subse quently the synthesis of diamonds was mastered in Sweden, the Netherlands, and Japan. In the Soviet Union the production of synthetic diamonds on a comercial scale began in 1961. The pressure in the process is of 3 Leipunskii, O. I.: Quoted from I. I. Shafranovskii, Diamonds, “ Nauka”, Moscow (1964).
Bonding. Infernal Structure of Solids
4t
the order of 100 000 atm and the temperature about 2000 °C. Synthet ic diamonds produced by this process are harder and stronger than natural diamonds and their industrial use is about 40 percent more efficient than that of natural ones. Another material of extreme hardness had been synthesized in a process similar to that of the diamond—the cubic boron nitride BN, which became known as borazon. It is harder than diamond and may be heated up to 2000 °C in atmospheric conditions. In its hexago nal modification boron nitride is similar to graphite—a white powder oily to the touch. From the theoretical point of view all solids should exhibit poly morphism provided the range of their stability is not limited by the processes of melting and sublimation. The existence of polymor phism is a direct consequence of the variation of the strength and the nature of the bonds in the crystal lattice caused by the changes in intensity of atomic motion and in the distance between them as a result of heating or of application of external pressure to the crystal. Close to absolute zero the stable structure should be that with the strongest bonds possible for the given atomic ensemble. In the case of tin, which belongs to Group IV of the Mendeleev periodic table, such structure is the diamond structure, in which every atom is bonded to 4 nearest neighbours by strong colvalent bonds. However, as the temperature is raised, those bonds, because of their strict directionality and rigidity, are easily destroyed by thermal motion, and already above 13.3 °C the flexible metallic structure formed with the aid of collectivized electrons becomes more favourable. This bond has its own stable crystal structure, the tetragonal bodycentred lattice. The transition from one modification to another is accompanied by the liberation or absorption of latent heat of transformation and is therefore a phase transition of the first kind. Such a transition involves the transformation of the crystal lattice and this fact togeth er with a low mobility of atoms in solids makes possible a practi cally infinitely long existence of a modification thermodynamically unstable in particular conditions. Diamond which can exist ages without turning into graphite—the stable modification in normal conditions—is a striking example of this point. Polymorphism is very important for practical purposes. Heat treatment of steels to obtain various properties, the production of stainless steels, the treatment of various alloys to obtain the necessary properties are all to a large extent based on the use of polymorphism.
42
Solid State Physics
§12 Imperfections and defects of the crystal lattice Mosaic structure. Numerous data obtained in the study of the struc ture of real crystals point to the fact that their internal structure is essentially not the same as that of an ideal crystal. To begin with, real crystals have a mosaic structure: they are made up of regular blocks which are only approximately parallel to one another. The dimensions of the blocks vary from 10~6 to 10“ 8 m and the angles between them from several seconds to tens of minutes. Because of the different orientation of adjacent blocks there is a transition layer between them in which the lattice changes its orientation Figure 1.25 Crystal lattice defects: (a) — Frenkel defects; N. Evidently, in such circumstances
Elements of Physical Statistics
89
the specific nature of fermions and bosons shall not be felt, since every particle has at its disposal a large number of different free states and the problem of several particles occupying the same state actually does not arise. Therefore the properties of the ensemble as a whole shall not depend on the nature of the particles that make it up. Such ensembles are termed nondegenerate, and condition (3.10) is the condition of nondegeneracy. If, however, the number of states G is of the same order of magni tude as the number of particles iV, that is if NIG « 1 (3.11) then the problem of how the states should be occupied, whether individually or collectively, indeed assumes much importance. In this case the nature of the microscopic particle is fully revealed in its effect on the properties of the ensemble as a whole. Such ensembles are termed degenerate. Degenerate ensembles are a unique property of quantum objects, since the parameters of state of such objects only change discretely with the result that the number of possible states G can be finite. The number of states for classical objects whose parameters change continuously is always infinite and they can form only nondegenerate ensembles. It should be pointed out that quantum mechanical objects too may form nondegenerate ensembles provided condition (3.10) is fulfilled (see Table 3.1). T able 3.1
Object Classical Quantum
Ensembles degenerate No Yes
nondegenerate Yes Yes
Classical and quantum statistics. Physical statistics that studies nondegenerate ensembles is termed classical statistics. It owes much to J. C. Maxwell and L. E. Boltzmann (the MaxwellBoltzmann sta tistics). Physical statistics that studies degenerate ensembles is termed quantum statistics. Owing to the effect of the particles’nature on the properties of a degenerate ensemble, degenerate ensembles of fer mions and bosons behave in essentially different ways. On this ground a distinction is made between two quantum statistics. Quantum statistics of fermions owes much to E. Fermi and P.A.M. Dirac (this, by the way, explains the origin of the term “ fermion” ). It is termed the FermiDirac statistics.
90
Solid State Physics
Quantum statistics of bosons owes much to S. N. Bose and A. Ein stein (hence the term “ boson” ). It is termed the BoseEinstein sta tistics. It follows then that quantum statistics deals only with quantum objects while classical statistics may deal both with the classical and the quantum objects. If we reduce the number of particles in an ensemble or increase the number of states, we shall eventually turn a degenerate ensemble into a nondegenerate one. In that case the ensemble shall be described by the MaxwellBoltzmann statistics no matter whether it contains fermions or bosons. Distribution function. What is the connection between the distri bution of the particles over particular states and the state of the en semble as a whole? To specify the state of an ensemble, for instance, of a gas of particles, one should specify its state parameters. To spec ify the state of each particle one should specify its coordinates and momentum components or its energy, which is a function of coordi nates and momentum. The two types of quantities are connected by the statistical distri bution function N ^ T{E)dE (3.12) which specifies the number of particles having an energy from E to E + dE in the system described by the state parameters pi and T . This function is termed complete statistical distribution function. To simplify notation the indices denoting the state parameters are usual ly omitted. The complete distribution function may be represented by the prod uct of the number of states g (E) dE per energy interval dE and the probability of occupation of those states by the particles. Let us de note the latter by / (E). Then N(E) dE = f(E) g(E) dE (3.13) The function f(E) is termed simply the distribution function. As was stated before it signifies the probability of the occupation of the respective states by the particles. If, for instance, 10 of 100 closely spaced states are occupied by particles (the total number of parti cles in the system being much greater than 100), the probability of occupation of such states will be equal to 0.1. Since on the average there is 0.1 of a particle per each state, we may take f(E) to be the average number of particles in a given state. Hence the problem of finding the complete distribution function of particles over the states is reduced to that of finding the function g(E) dE, which describes the energy distribution of the states, and the function f(E) which determines the probability of their occupa tion. We start by determining the function g(E) dE.
91
Elements of Physical Statistics
§25 The number of states for microscopic particles Concept of phase space of a microscopic particle and quantization. In classical mechanics the state of a particle is determined if its three coordinates (x, y, z) and three components of its momentum (px, Pyi Px) are specified. Let us imagine a sixdimensional space with the coordinate axes x, y, z, p x, p y, p z. The state of the particle at every moment of time will be described by a point (x, y, z, p x, p y, Pz) Such space is termed phase space and the points (x, y, z, p x, p y, p z) are termed phase points. The quantity AT = ATyATp = dx dy dz dpx dpy dpz
(3.14)
is termed an element of the phase space. Here ATv = dx dy dz is an element of volume in coordinate space and ATp = dpxdpydpz an element of volume in momentum space. Since the coordinates and the momentum components of a classical particle may change continuously, the elements ATv , ATp and with them the element AT as well can be chosen as small as desired. The potential energy of a system of noninteracting particles not acted upon by an external field is zero. Such particles are termed free. For such particles it is convenient to use a threedimensional momentum space instead of the sixdimensional phase space. In this case the element ATv is simply equal to the volume V in which the particles move, because no additional restrictions are placed on them. The division of the phase space into elements of volume is not quite so simple if the particle in question is an electron or some other mi croscopic object possessing wave properties. The wave properties of such particles make it impossible, in accordance with the uncertainty principle, to distinguish between two states, (x, y, z, p x, p y, p z) and (x + dx, y + dy, z + dz, p x + dpx, p y + dpy, p z + dpz), if the product dx dy dz dpx dpy dpz is less than hs. Since this product rep resents an element of volume in sixdimensional phase space, it follows from the above that different quantum states shall corre spond to different elements of volume in this space only if the size of those elements is no less than h3. Therefore quantum statistics makes use of an elementary cell in the sixdimensional space with the volume AT = ATv ATp = h3 (3.15) The element of the threedimensional momentum space for free par ticles for which ATv = V is ATp = h3IV
(3.16)
Solid State Physics
92
Each element of this kind has corresponding to it a definite quantum state. The process of dividing the phase space into cells of finite size (ft3 or ft3/F) is termed quantization of phase space. Density of states. We wish to calculate the number of states of a free particle in the energy interval from E to E + dE. To this end draw two spheres of the radii p and p dp in the momentum space Figure 3.1 C a lcu la tin g the num ber o f sta tes o f a m icr o s co p ic particle.
h i E E+dE
Px (Figure 3.1). There is a spherical layer with the volume of 4np*dp contained between the spheres. The number of phase cells contained in this layer is (3.17) Since there is one particle state to correspond to every cell the number of states in the interval dp between p and p + dp is g{p)dp = —
PUp
(3.18)
For free (noninteracting) particles
Using these relations to express p and dp and substituting the results into (3.18), we obtain g (E ) dE = ^ ~ (2m)3'2 V E dE
(3.19)
93
Elements of Physical Statistics
This is the number of states of a free particle in the energy interval (E, E f dE). Dividing the right and the lefthand sides of (3.19) by dE, we obtain the density of states, g(E), which specifies the num ber of states of a microscopic particle per unit energy interval: g(E) = ^  ( 2 m ) m V E
(3.20)
It follows from (3.20) that as E increases the density of states rises in proportion to Y E (Figure 3.2). The density of states depends, besides, on the particle’ s mass and increases with m. Figure 3.2 E n ergy depen den ce o f den sity o f states.
In case of the electrons each phase cell corresponds, to be exact, not to one but to two states, each distinguished by its spin. They are termed spin states. Therefore in case of the electrons the number of states (3.18) and (3.19) and the density (3.20) should be doubled: g(p)dp = 2%Pp>dp
(3.21)
g (E) d E = ^  ( 2 m ) 312 V E d E
(3.22)
g(E) = ^  ( 2 m f 2 V E
(3.23)
Condition of nondegeneracy for an ideal gas. Integrating (3.20) with respect to energy from 0 to E, we obtain the number of particle states contained within the energy interval (0, E): G = ^  ( 2 m f l 2~ E 312 Setting E = (3/2) kBT, we obtain G * * y ( 2nmh**T y n
94
Solid State Physics
Substituting this expression into (3.10), we obtain the condition for nondegeneracy:
where n = NIV is the number of particles per unit volume. Consider some molecular gas, for instance, nitrogen in normal con ditions. For it n & 1026 m “ 3, m = 4.5 X 10~26 kg, and kBT = 4 X X 10~21 J. Substituting the figures into the lefthand side of (3.24), we obtain nh3(2nmkBT)~3/2 » 10“ 6, which is much less than unity. Accordingly, the molecular gases are normally nondegenerate and must be described with the aid of the MaxwellBoltzmann classical statistics. Consider now the electron gas in metals. For it n « 5 X 1028 m “ 3, m = 9 X 10~31 kg. For such values of n and m the electron gas turns out to be nondegenerate only at temperatures above 105 K; the lefthand side of (3.24) for such temperatures diminishes to less than unity (at T = 105 K it is approximately 0.5). Therefore in practice the electron gas in metals is always degenerate and on account of this should be described with the aid of the FermiDirac statistics. It follows from (3.24) that a nondegenerate state of a gas can be realized not only by raising its temperature but by reducing its con centration n as well. For n « 1022 m ~3 the lefthand side of (3.24) for electrons at normal temperatures is approximately 10~3 and the electron gas becomes nondegenerate. Such (and smaller) concentra tions of the electron gas are found in some semiconductors. In such semiconductors termed nondegenerate, the electron gas is nondegen erate and is described by the classical MaxwellBoltzmann statistics. Let us try now to find the distribution function f{E). The form of this function depends in the first instance on whether the gas is de generate or nondegenerate. In the case of a degenerate gas the impor tant point is whether the gas consists of fermions or bosons. Let us start with a nondegenerate gas whose distribution function f(E) is independent of the particles’nature.
§26 Distribution function for a nondegenerate gas Appendix I contains an elementary derivation of the distribution function for a nondegenerate gas. It is of the following form: f(E) = eiv E)lhKT
(3.25)
where kB is Boltzmann’ s constant, and fx the chemical potential. Calculations give the following expression for li of a nondegenerate
95
Elements o f Physical Statistics
gas: P26) Substituting it into (3 25) we obtain:
We would like to remind again that /M(i?) dE expresses the proba bility of occupation of the states in the energy interval (E , E + dE); the term for it is the MaxwellBoltzmann distribution function. Figure 3.3 Distribution functions for nondegenerate gas: (a)—the MaxwellBoltzmann distribution function expressing the average density of state occupation by particles; (b)—the complete MaxwellBoltzmann distribution function.
Figure 3.3(a) shows a graph of the function It has a maxi mum at E == 0 and asymptotically approaches zero as E oo. This means that the lower energy states have the greatest probability of occupation. As the energy of a state increases its probability of oc cupation diminishes steadily. Multiplying /M(i?) by the number of states g(E) dE [see (3.22)], we obtain the complete distribution function of particles over the energy N (E) dE = ^ j
(2 m )3/Y
/fta V
E/AB T
y j ? dE
(3.28)
or N (E )d E = — 2 .N — j >  E/hBT V W d E V ’ 1f n ( k BT )*
(3.28') V
96
Solid Stafe Physics
It is termed the complete MaxwellBoltzmann distribution function• Figure 3.3(b) shows the graph of this function. Because of the factor ]/ E its maximum is displaced to the right of the origin. Knowing the distribution function /m(^)> we may easily find the laws of distribution of the particles over the momentum, N(p) dp, and over its components, N(px, p y, p z) dpxdpydpz, over velocity, N(v) dv, and over its components N(vx, vy, vz) dvxdvuduZf over one of the components of velocity, say N(ux) dvx, etc. Those distributions are shown below n ( P) =
M
(2n mkBT ) 3/2
. w ^ v y
(3.29) (3.30)
N(Px, p„
v
N (v „
Vy,
Pz)= ' VZ)
N
(2nm kBT ) m
= N
e ^ +pl +pVl(2mhBT>
T)3/\  m^ +Pl +v? n2hBr>
(3.31) (3.32) (3.33)
The reader is requested to obtain those results himself.
§27 Distribution function for a degenerate fermion gas The distribution function for a degenerate fermion gas was first ob tained by Fermi and Dirac. It is of the following form: fr {E) = (eE~m bt +1)»
(3.34)
An elementary derivation of this expression is presented in Appen dix II. Here, as before, p, denotes the chemical potential, which in the case of a degenerate fermion gas is termed the Fermi level. Formula (3.34) shows that for E = p, the distribution function h{E) = 1/2 at any temperature T =£ 0. Therefore from the statis tical point of view the Fermi level is a state whose probability of occupation is 1/2 . The function (3.34) is termed the FermiDirac function. To obtain a clear picture of the nature of this function one should consider the degenerate electron gas in metals at absolute zero. Electron distribution in a metal at absolute zero. Fermi energy. The metal is a sort of a potential trough for free electrons. To leave it the electron should have work performed on it against the forces retaining it in the metal. Figure 3.4 shows the diagram of such a
Elements of Physical Statistics
97
potential trough. The horizontal lines denote energy levels which the electrons may occupy. In compliance with the Pauli exclusion prin ciple there may be two electrons with opposite spins on each such level. For an electron gas of N electrons the last occupied level will be the A72 level. This level is termed the Fermi level for a degenerate Figure 3.4 Schematic representation of a metal as a potential trough for free electrons.
electron gas. It corresponds to the maximum kinetic energy' E F an electron in a metal may possess at absolute zero. This energy is termed the Fermi energy. Thus at absolute zero all states with the energy E < EF are oc cupied by electrons and all states with the energy E > EF are free. In other words, the probability of occupation of a state with the energy E < E F at T = 0 K is unity and the probability of occu, pation of a state with the energy E > EF is zero: /F (E) = 1 for = 0 for
E E
f
(3.35)
To obtain this result from (3.34) one should assume that at T = 0 K the chemical potential of the electron gas measured from the bottom of the potential trough is equal to the Fermi energy E F: P0 = Indeed, setting in (3.34) p,=Z?Ft we obtain /P (£) = (e(E" EF>/ftBT+ i)i
(3.36) (3.37)
If E < E f , then e(EEF)/ftBr o at f = 0 K and /F = 1; if E > Z?F, then e(E~EF)/kBT oo at T = OK and /F = 0. Figure 3.5(a) shows the graph of the FermiDirac distribution func tion at absolute zero. It has the shape of a step terminating at E = Ef , 70885
98
Solid State Physics
Multiplying (3.35) by the number of states g(E) dE [see (3.22)], we obtain the complete FermiDirac distribution function at absolute zero: N {E )dE = ^f(2 m )*i*V ~ E dE
(3.38)
because/F = 1 in the energy interval (0, EF). The graph of the func tion is presented in Figure 3.5(b), where the area of the occupied states is shaded. Figure 3.5 The distribution function for degenerate fermion gas: (a) —the FermiDirac distribution function for T = 0 K, (b) —the complete FermiDirac distribution function for T = 0 K.
Integrating expression (3.38) from 0 to E F, we obtain N = ^ E \ ' 2(2i»)s/2 whence the Fermi energy EF may be easily obtained
(» ■ « » where n = N/V is the concentration of electron gas in the metal. Knowing the energy distribution function of the electrons, we may easily calculate the average energy of the electrons at absolute zero, E 0:
3
in
3h ?
/ 3 n \ 2/3
* 0= 5  £ F = io ^ ( & r )
/q/rk\
(340)
Lastly, knowing E F and E 0, we can calculate the maximum velocity vF and the effective velocity i;eff (corresponding to average energy) of free electrons in a metal at absolute zero: /
2Ef IT '
v*t t = V
i/ * 2 E q IT
(3.41)
99
Elements of Physical Statistics
Table 3.2 shows the Fermi energy E F, the average energy E 0r the maximum and effective velocities of free electrons at absolute zero for some metals. The last column contains the Fermi temperature determined from the relation T F = E F!kB
(3.42)
This is the temperature at which a molecule in a normal nondegen erate gas would have the energy of thermal motion (3/2) kBT equal to the Fermi energy E F multiplied by 3/2. Table 3.2
Metal
EF (eV)
*0 (eV)
Copper Lithium Silver Sodium
7.1 4.72 5.5 3.12
4.3 2.8 3.3 1.9
vF (106m/s) 1.6 1.3 1.4 1.1
y e ff
(106 m/s) 1.25 1 1.1 0.85
Tp
(104 8.2 5.5 6.4 3.7
It may be seen from Table 3.2 that Fermi temperatures are so high that no metal can exist in a condensed state. It should be stressed that although the Fermi energy represents the kinetic energy of translational motion of free electrons it is not the energy of their thermal motion. Its nature is purely quantum me chanical and is due to the fact that electrons are fermions satisfying the Pauli exclusion principle. Temperature dependence of the FermiDirac distribution. When the temperature is raised, the electrons become thermally excited and go over to higher energy levels. This causes a change in their distri bution over the states. However, in the range of temperatures in which the energy of their thermal motion, kBT, remains much less than EF only the electrons in a narrow band about approximately kBT wide adjoining the Fermi level may be thermally excited (Fig ure 3.6(a); the excited states are shaded). The electrons of the lower levels remain practically unaffected because the energy of thermal excitation kBT is not enough to excite them (to transfer them to levels above the Fermi level). As a result of thermal excitation some of the electrons with an ener gy less than EF are transferred to the levels with energies greater than E F and a new distribution of electrons over the states is estab lished. Figure 3.6(b) shows the curves of the electron distribution over the states for T — 0 K (curve 1) and for T > 0 K (curve 2). It can be seen that the rise in temperature causes the original distribution to smear to a depth of kBT with a “ tail”BC appearing to the right of EF. The higher the temperature the greater the change in the dis
100
Solid State Physics
tribution function. The tail BC itself is described by the Maxwellian distribution function. The shaded areas in Figure 3.6(b) are proportional to the number of electrons transferred from the states with E < i ? F (the area ADB) to the states with E > EF (the area E FBC). Those areas are equal since they represent the same number of electrons. Let us make an approximate estimate of this number, AN. There are N/2 energy levels inside the interval (0, E F), where N is the num ber of free electrons in the metal. To simplify the problem we may Figure 3.6 Temperature dependence of the FermiDirac distribution function: (a)—thermal excitation of electrons; (b)—the FermiDirac distribution function for T > 0 K.
N
assume that these levels are equidistant, the separation being Ac = = E FI(NI2) = 2EF/N. Only the electrons in the band kBT wide just below E f (Figure 3.6(a)) are thermally excited. There are kBT/ Ae = kBTNl{2EF) levels inside this band occupied by 2JsBTNI(2EF) = kBTN!EF electrons. Assuming that not more than a half of those electrons go over the Fermi level, we obtain the fol lowing approximate relation for AA: AN~  m N
At room temperature kBT « 0.025 eV, E F = 310 eV, therefore AN/N < 1 percent; at T = 1000 K we find that AN/N « 12 per cent. Hence in all the temperature range in which the electron gas in a metal is degenerate its distribution is close to that at absolute zero. Accordingly, only a negligible fraction of the electrons close to the Fermi level are thermally excited. At room temperature this fraction is less than 1 percent of the total number of conduction electrons. The laws governing the distribution of the electrons in metals dis cussed above remain valid practically in all cases, because in all the
101
Elements of Physical Statistics
temperature range in which the existence of metals in the con densed state is possible the electron gas remains degenerate. Consider the temperature dependence of the chemical poten tial. Integrating the complete FermiDirac distribution function f?(E) g(E) dE over energy, we obtain the total number N of free electrons in a metal: OO
OO
N = ( f F(E)g(E)dE^ —
(2m)^2 j E'l'dE (e 1 (3.47) It follows from (3.47) that for a nondegenerate electron gas in which condition (3.46) is satisfied — p should be a positive quantity con siderably greater than kBT:  \ i > kBT
(3.48)
The chemical potential p should be negative and greater than kBT in absolute value. If the condition (3.46') is fulfilled, unity in the denominator of the FermiDirac function can be neglected and the following expresFigure 3.7 Temperature dependence of energy, pressure, and the square of effective velocity of electrons in a metal.
h p .eff Region of degenerate state Re g i o n of nondegencrate state
0
7p
r
sion for the distribution function of a nondegenerate electron gas may be obtained: f (E) = e'llk^Te~E/kbt
(3.49)
Comparing (3.49) with (3.25), we see that a nondegenerate electron gas like every other nondegenerate gas is described by the MaxwellBoltzmann distribution function. The electron gas in metals, where the free electron concentration is always very high («1028 m “ 3), is always in a degenerate state de scribed by the FermiDirac distribution function. A nondegenerate electron gas is a feature of the intrinsic {pure) and weakly doped semiconductors, which are the mainstay of modern semiconductor electronics. The concentration of free electrons in such semiconductors is substantially less than in metals, varying from 101610lfJ to 10231024 m ~3 depending upon the concentration of elec trically active impurities. The nondegeneracy condition (3.10) re mains valid for such concentrations and the electron gas is nonde generate. In conclusion, to illustrate the drastic difference in the behaviour of the ideal nondegenerate gas obeying the MaxwellBoltzmann sta
103
Elements of Physical Statistics
tistics and of the degenerate electron gas described by the FermiDirac statistics, we would like to cite some of their properties (Table 3.3). T able 3.3
Gas Parameters
nondegenerate
II
E TK
E ^ k BT
0 K
"eft
TK
_
, /"
v 0
Ik
asp II
TK
~
3
F
* T hr
0
OK
P
co uo
o 1^
0
OK
degenerate
ye f t =
3JcbT m
*
106 m ''s
vcH » «&r p° = £0 » 1010 Pa o
p »p°
It follows that average energy E, effective velocity vCff and pres sure p of a nondegenerate ideal gas are functions of temperature that vanish at absolute zero. At the same time E, i?eff, and p of a degen erate electron gas are very large already at absolute zero and are prac tically independent of temperature (Figure 3.7). This points to the fact that, as noted above, E, yeff, and p of a degenerate electron gas are for the most part not of thermal origin, the contribution of the thermal electron motion to these quantities being negligible.
§28 Distribution function for a degenerate boson gas In contrast to the electrons, which satisfy the Pauli exclusion prin ciple, the bosons can occupy both the free states and the states already occupied by other bosons the more readily the greater the occupancy of the latter. The distribution function of bosons over the states was first ob tained by Bose and Einstein. It is of the following form: /Bose(^) = (e(B" ll)/ftBT l )1
(3.50)
104
Solid State Physics
(An elementary derivation of this expression is given in Appendix III). It is termed the BoseEinstein distribution function. Let us use it to describe the state of a photon gas. Suppose that a cavity inside a black body at a temperature T is filled with equilibrium thermal radiation. From the quantum mechan ical point of view this radiation may be regarded as consisting of an enormous number of photons constituting a photon gas. The photon’ s spin is s — 1. Therefore photons are bosons, which implies that the photon gas should satisfy the BoseEinstein distribution. The photons have some peculiarities as compared w7ith other bo sons, for instance, the helium nucleus, vHe. (1) The rest mass of a photon is zero. (2) All photons move with the same speed equal to that of light, c, but can have different energy E and momentum p ; E and p depend on the photon’ s frequency: E = hv = ho), p = hv/c = hw/c (3.51) where ft = hl2n and (o = 2jtv. It follows from (3.51) that E = pc
(3.52)
(3) The photons do not collide with one another. Therefore an equilibrium distribution in a photon gas can be established only in the presence of a body capable of absorbing and emitting photons. The walls of the cavity in which the radiation is contained may serve as an example of such a body. The transformation of a photon of one frequency into a photon of another frequency takes place in the pro cesses of absorption and subsequent emission. (4) The photons may be generated (in the act of emission) and an nihilated (in the act of absorption) in any numbers. Therefore the number of photons in a photon gas does not remain fixed but depends on the state of the gas. For specified values of V and T the photon gas in a state of equilibrium contains so many photons N 0 as are needed for the energy of the gas to be at its minimum. This makes it possible to express the condition for the equilibrium of the photon gas in the form:
(w),.r=°
(3M>
Since according to (3.8) (dE/dN)v,r = p the equilibrium condition (3.53) means that p = 0. Hence the chemical potential of an equi librium photon gas is zero. For a nondegenerate gas the chemical potential is negative and has a relatively great absolute value. The fact that for the photon gas p = 0 means that such gas is always degenerate. Setting p = 0 in (3.50), we obtain the distribution function for the photon gas: fp (E) = (eE/ftBT — l)i = (eha/hBT— l)i (3.54)
105
Elements of Physical Statistics
This formula was first obtained by Max Planck and is termed the Planck formula. It represents the average fraction of photons having the energy E == So>. Using this formula, we may easily formulate the law for the energy distribution in the spectrum of a black body. The following expression can be obtained for the energy density of the radiation of such a body: 2h
CO
3
“ JtC3 e tM/kBr
/ Q
_ {
rr\
(3.5d)
The readers are requested to derive this formula themselves mak ing use of (3.54) and (3.18).
§29 Rules for statistical averaging As was already stated, to specify the state of an ensemble one should specify its state parameters. To specify the state of a particle one should specify the values of its coordinates and momentum compo nents. The problem of going over from the parameters of the individual particles to the state parameters characterizing the ensemble involves the problem of transition from the dynamical laws describing the behaviour of the individual particles to the statistical laws describ ing the behaviour of the ensemble. To effect such a transition it is necessary to perform the averaging of the characteristics of motion of the individual particles assuming the chances of all the particles belonging to the ensemble to be identical. The state parameters of the ensemble are expressed in terms of the averaged parameters of the individual particles belonging to the ensemble. To make the rules of averaging apparent let us consider an ensemble of N identical particles each of which is capable of assuming one of the discrete set of energy values: E t, E 2, . . ., E m. Choose an arbitrary moment of time and note the energy every particle has at that moment. We obtain as a result a set of numbers N(Ei) express ing the number of particles having the energy E t. To determine the average energy E of the particles we add up the energies of all of them and divide the sum by the number of particles. The total number of particles is N = y\T= i M ) , and the sum of their energies is N{Et) E t. Therefore
2
i=
E iN (Ei) 1________________
m
2 N (El)
i= l
(3.56)
106
Solid State Physics
The average value E obtained in this fashion is termed an ensemble
average.
If the particle’ s energy assumes a continuous set of values, the practice is to count the number of particles having an energy lying within an interval (E , E + dE) instead of the number of particles having an exact value of energy. The average energy will then be oo $ EN(E) dE
1 = 4 
(3.57)
J N(E) dE
6
Such averaging may be performed for any physical quantity M that is a function of the coordinates and the momenta of the parti cles making up the ensemble. If M is continuous, oo
$ MN(M) dM
¥ = 4 
(3.58)
$ N(M) dM
b Let us determine the average energy of the particles of an ideal nondegenerate gas. According to (3.57) and (3.28), we have oo
$ EN(E) dE
E = OO 
—  f eE/ftBr£.V2 dE = 3 ig T
(3.59)
$ N(E)dE
6
The results of the calculations of the average values of the velocity, of a velocity component, of the effective velocity, and of its compo nent for the particles of an ideal gas are presented thus:
—  ( ¥ ) “* The reader may for the sake of practice perform these calculations himself.
4 Thermal Properties of Solids
§30 Normal modes of a lattice The atoms of a solid take part in thermal vibrations around their equilibrium positions. Because of a strong interaction between them, the nature of those vibrations turns out to be extremely complex and an accurate description of it presents enormous difficulties. There fore approximate methods and various simplifications are used to solve this problem. Instead of describing the individual vibrations of the particles the practice is to consider their collective motion in the crystal, which is a spatially ordered structure. This simplification is based on the fact that powerful bonds immediately transmit the vibrations of one particle to other particles and a collective motion in the form of an elastic wave involving all the particles of the crystal is excited in it. Such collective motion is called the normal mode of a lattice. The number of normal modes coincides with the number of degrees of freedom, which is 37V if TV is the number of particles constituting the crystal. Figure 4.1(a) represents a onedimensional model of a solid—a linear chain of atoms separated by a distance a and able to vibrate in the direction perpendicular to the chain. Such a chain may be re garded as a string. If the ends of the chain are fixed, the fundamental mode corresponding to the lowest frequency co]nin is represented by the standing wave with a node at each end (Figure 4.1(b), curve 1). The second mode is represented by the standing wave with an addi tional node in the centre of the chain (curve 2). The third mode, or third harmonic, is represented by the standing wave with two addi tional nodes that divide the chain in three equal parts (curve 5), etc. The length of the shortest wave in such a chain is evidently equal to twice the distance between the atoms of the chain (Figure 4.1(c)):
^min = 2a (4.1) The corresponding maximum freguency (omax is wmax — 2jtl?/A/min = zivl a (4.2) where v is the velocity of wave propagation (of sound) along the chain. 107
108
Solid State Physics
This maximum frequency is a parameter of the chain’ s material and is determined by the interatomic distance and the velocity of wave propagation. Should we set a = 3.6 X 10“10 m (the lattice parameter of copper) and v = 3550 m/s (the velocity of sound in copper) we would obtain comax « 3 X 1013 s 1, which corresponds to the frequency of atomic vibrations in a solid.
J±t
Figure 4.1 Normal modes of a linear chain made up of identical atoms: (a)—linear chain; (b)—normal modes of the chain; (c)—normal modes of the chain corresponding to shortest wavelength (to highest frequency); (d)—dispersion curves expressing dependence of normal mode frequency on wave vector.
To describe wave processes one usually uses the wave vector q whose direction coincides with that of wave propagation and whose absolute value is q = 2n/K (4.3) It follows from (4.2) that 2n/k = co/v. Therefore*6 q = (o/y, or co = qu
(4.4)
6 The phase velocity v, which enters (4.4), is itself a function of the wave vector q and for a linear chain of atoms bonded by elastic forces is expressed by the following relation: sin (qa/2) v = v0 (4.4') qa/2 where u0 is the velocity of wave propagation in a continuous string for which a = 0. It follows from (4.4') that for a constant a the velocity v is practically independent of q and is approximately v0 only in the range of small q's, where [sin (qa/2)]/(qa/2) « 1. In this range co increases approximately in proportion to q (Figure 4.1(d)). As q increases the value of [sin (qa/2)]/(qa/2) steadily dimin ishes and for q = n/a tends to 2/n. This causes the dispersion curve co(q) to flatten out, so that for q = n/a it runs parallel to q.
109
Thermal Properties of Solids
Figure 4.1(d) shows the dependence on wave vector q of the fre quency of normal modes in a linear chain made up of atoms of one kind. As q increases from 0 to nla the frequency of the normal modes rises, reaching the maximum value comax = nvla for q = nla, that is, for X = 2a. Curves of this type expressing the dependence of the vibration frequency on the wave vector (the wavelength) are termed dispersion curves. Figure 4.2 Normal modes of a chain made up of atoms of two kinds: (a)—arrangement of atoms in the chain; (b)—acoustic modes; (c)—optical modes; (d)—dispersion curves for acoustic and optical modes; (e)—linear lattice with a basis in which optical and acoustic modes are present. 2a
M.
m
Af
(a)
U)
  * 3 «w
4

V

y "V hA
1 1
v
—ti/2 a
12
12

12
ti/2 a
(e)
12 (d)
Consider now a chain made up of atoms of two kinds placed in a regular sequence one after another (Figure 4.2(a)). Denote the mass of the heavier atoms by M and that of the lighter atoms by m. Two types of normal modes can be present in such a chain, as is shown in Figure 4.2(b, c). The modes 4.2(b) are quite identical to the modes of a uniform chain: the phases of the neighbouring atoms are practically the same. Such vibrations are termed acoustic modes, since they in clude the entire spectrum of the acoustic modes of the chain. For them coac = 0 for q = 0. They play a decisive part in determining the thermal properties of the crystals such as heat capacity, heat conductivity, thermal expansion, etc. In case of normal modes shown in Figure 4.2(c) the phases of the neighbouring vibrating atoms are opposite. Such modes can be treat
110
Solid State Physics
ed as the relative vibrations of two interpenetrating sublattices, each made up of atoms of one kind. They are termed optical modes, since they play a decisive part in the processes of interaction of light with crystals. Figure 4.2(d) shows the dispersion curves for the acoustic (1) and optical (2) normal modes of a chain made up of atoms of two kinds. In contrast to an acoustic mode, whose frequency rises with the wave vector reaching the maximum value at qmax = jt/(2a), the maximum frequency of an optical mode corresponds to q = 0 ; with the increase in q the frequency of an optical mode falls off to its minimum at *7max = Jt/(2fl). The optical vibrations are possible not only in a chain made up of atoms of different kinds, but in a complex chain made up of two, or more, interpenetrating chains containing atoms of one kind, as shown in Figure 4.2(e). Unit cell of such a complex chain contains two atoms. The optical modes are the result of the relative vibrations of two sublattices.
§31 Normal modes spectrum of a lattice One of the principal problems of the theory of lattice vibrations is the problem of the frequency distribution of normal modes. Consider now the simplest case of the normal modes in a linear atomic chain (see Figure 4.1). The wavelengths of the normal modes in such a chain are Xn = 2L!n
(n = 1, 2, 3, . . ., N)
(4.5)
where L is the length of the chain, and N the number of atoms in it. The number of normal modes z having the wavelength [equal to or greater than Xn will evidently be n: z — n — 2L/Xn In the same way the number of standing waves in a threedimen sional crystal of volume V (for instance, in a cube with edge L and volume L3) having the wavelength equal to or greater than X should be z
= (2u x y = 8m3
A more accurate calculation yields z = 4nV/X3
(4.6)
Since X = 2ju;/(d, it follows that Z “ 2n2v3 00
(4.7)
Ill
Thermal Properties of Solids
Differentiating this expression, we obtain dz = g (w) d© = — 5©2cZg)
(4.8)
Formula (4.8) expresses the number of normal modes per frequency interval (co, co + dco). The function (49> determines the density of the normal vibrations in do of the spectrum, that is their spectrum. The function g(o) is termed spectral distri bution function of normal modes. Since the number of normal vibrations in a lattice is 3N, the func tion g(o) should satisfy the following normalization condition: "d ^ g (co) dco == 37V o
(4.10)
where o D is the maximum frequency limiting the spectrum of nor mal modes from above. Substituting (4.9) into (4.10) and integrating, we obtain ,°3 37V Zn*v3
(4.11)
2 pr N \j 1/3 (0D = u fl a6ji2
(4.12)
Hence
The frequency coD is termed the Debye frequency and the temperature 0 = to n
kB
(4.13)
the Debye temperature. Table 4.1 shows the Debye temperatures of some chemical elements and compounds. At the Debye temperature the entire vibration spectrum is ex cited in the solid, including the one with the maximum frequency g)d Accordingly, any further rise in temperature (above 0) shall not be accompanied by the appearance of new normal modes. In this case the role of the temperature is to increase the intensity of each of the normal modes with a resultant increase in their average energy. Temperatures T > © are usually referred to as high temperatures* Substituting v3 from (4.11) into (4.9), we obtain g(o) = 9 N %
(4.14)
112
Solid State Physics
Table 4.1 Element
e (K)
A1 Ag Au Be Bi C (diamond) Ca CaF2 Cd Co Cr Cu
418 225 165 1160 117 1910 219 474 300 445 402 339
Element Fe Ge Hg In KBr KC1 La Mg Mo NaCl Nb Ni
0 (K)
Element
0 (K)
467 366 (6090) 109 174 227 132 406 425 320 252 456
Pb Pd Pt Si Sn (gray) Sri (white) Ta Ti T1 V W Zn
94.5 275 229 658 212 189 231 278 89 273 (379) 308
§32 Phonons Each normal mode carries with it some energy and momentum. Oscillation theory contains the proof of the fact that the energy of a normal mode is equal to the energy of an oscillator with a mass equal to the mass of the vibrating atoms and the frequency of the normal mode. Such oscillators are termed normal. Denote the energy of the ith mode characterized by the frequency co j by E tn.m. It is equal to the energy E tn.0 of a normal oscillator of the same frequency co*: E tn.m = E tn.0. The total energy of the crys tal in which all the 3N normal modes have been excited is 3
E =
N
1
E{ n.o
Hence the total energy of the crystal made up of N atoms taking part in coupled vibrations is equal to the energy of 3N independent normal harmonic linear oscillators. In this sense a system of N atoms whose vibrations are interconnected is equivalent to a set of 3N nor mal oscillators and the problem of calculating the average energy of such a system is reduced to a simpler problem of calculating the av erage energy of normal oscillators. It should be pointed out that normal oscillators have nothing in common with real atoms except the mass. Every oscillator represents one of the normal modes of the lattice in which all the atoms of the crystal take part vibrating with the same frequency co. The energy of a quantum oscillator is, as is well known, expressed by the relation E n = (n + 1/2) heo
(n = 0, 1, 2, . . .)
(4.15)
113
Thermal Properties of Solids
where od is the oscillator’ s vibration frequency, and n the quantum number. Figure 4.3 shows the energy spectrum of a linear harmonic oscil lator. It consists of a set of discrete levels spaced at an interval of /ko. Since i?n.m = ^n.o» the expression for the energy of the normal modes of a lattice should be (4.15) and the energy spectrum should coincide with that shown in Figure 4.3. The minimum portion of energy that can be absorbed or emitted by the lattice in the process of thermal vibrations corresponds to Figure 4.3 Energy spectrum of linear harmonic oscillator.
the transition of the normal mode being excited from the given energy level to the adjacent level and is equal to eph = /ko (4.16) This portion, or quantum, of energy of thermal vibrations of the lattice is termed a phonon. The following analogy may help to clear up the point. The space inside a black body is filled with equilibrium thermal radiation. From the quantum mechanical point of view such radiation is treat ed as a gas made up of the light quanta, or photons, whose energy is e = ftco = hv and whose momentum is p = hca/c = h/Xy where c is the velocity of light, and X its wavelength. The field of elastic waves in the crystal may be treated similarly as a gas made up of quanta of the normal modes of the lattice, or of phonons having the energy eph = h® = hv and momentum p vh = fico/v = h/X = Kq
(4.17)
where v is the velocity of sound, and X the length of the elastic wave.
114
Solid State Physics
From this point of view a heated crystal may be likened to a box filled with phonon gas. The analogy may be extended. Phonons are described by the same BoseEinstein distribution function (3.54) as photons: /vf
eW *BT_ !
eh(*/kBT 1
Depending on the intensity of excitation of the normal mode it can “ emit”a definite number of phonons. Thus, if some normal mode Figure 4.4 (a)—phonon energydistribution function; (b)—illustration of the fact that normal modes excited in the lattice at temperature T are mainly those with energy^quanta hm < k BT.
E 1
1 (DP
©
/
CDc
(b)
was excited to the third level (Figure 4.3), its energy became E 3 = = (3 + 1/2) ft©; this means that the particular normal mode has “ generated”three identical phonons each with an energy of ft©. Figure 4.4(a) shows the graph of the phonon energy (frequency) distribution function f{E). We see that for a given temperature T all normal modes in a lattice up to those with the energy ft© « kBT are excited; practically no quanta of higher frequencies with the energy ft© > kBT are excited. This is quite evident from Figure 4.4(b). Horizontal strokes here denote energy spectra of normal modes with the frequencies ©x = kBT/(8h), © 2 = kBT/(4h), cd3 = = kBT/(2h), ©4 = kBT/H, and © 5 = 2kBT/h; the level correspond ing to kBT is shown by a dotted line. It follows that for a given tem perature T the mode with the frequency ©x is excited approximately to the 8th level. As was stated before, this means that this normal mode “ generates” eight identical phonons with the energy S©x =
Thermal Properties of Solids
115
= kBT!& each. The normal mode with the frequency co2 is excited approximately to the 4th level, that with the frequency cog to the second, and that with the frequency o)4 (whose quantum of energy is ^o)4 = kBT) to the first. At the same time the vibration co5 is rarely excited at T because its excitation energy ftco5 is too high. The exci tation of still higher frequencies is a much more rare event. Therefore we can say that approximately only the vibrations with frequencies not greater than 00 corresponding to the energy hco « kBT are excit ed in a solid at temperatures T
1 28
Solid State Physics
where k is the mean free path of the molecules, v their thermal ve locity, and Cv the heat capacity of the gas. Let us apply this formula to the phonon gas substituting for Cv the specific heat of the crystal (the phonon gas), for % = Xvh the mean free path of the phonons, and for u the velocity of sound (the phonon velocity). We obtain the following expression for the lattice heat conductivity: ^lattice = vk^CylS (4.53) Substituting k ^ into (4.53) from (4.51), we obtain ^lattice OC
:, 2(4.54) “ pne In the high temperature range, in accordance with (4.37), nph OC T; hence ^ la ttice a  p 
(4.55)
Since Cv in this range is practically independent of T, the lattice thermal conductivity should be inversely proportional to the absolute temperature, which is in qualitative agreement with experiment. Formula (4.55) also includes the anharmonicity factor g and the sound velocity v, which depend substantially on the rigidity of the bonds between the particles of the solid. Bonds of lesser rigidity correspond to lower v's and to greater g's, since the weakening of the bonds makes for greater thermal vibration amplitudes (for a specified temperature) and for greater anharmonicity. Both those factors should, according to (4.55), bring about a reduction in latticeThis conclusion is supported by experiment. Table 4.2 presents the values of sublimation heat (?s, which is a measure of bonding energy, and of the lattice heat conductivity la t tic e for some covalent crystals with the diamond lattice: diamond, silicon, and germanium. Table 4.2
Substance
Qs (105 J/mole)
c)riattice (W/(mK))
Diamond Silicon Germanium
71.23 46.09 37
550 137 54
We see that the decrease in the bond energy from the value of diamond to that of silicon and, finally, germanium is accompanied by a noticeable decrease in the lattice heat conductivity. A more detailed analysis shows that la t t ic e is also strongly dependent of the mass M of the particles, being less for greater M ’ s. This to a large extent accounts for the fact that the lattice heat conductivity of the
Thermal Properties of Solids
129
lighter elements occupying the upper part of the Mendeleev periodic table (B, Ct Si) is of the order of tens or even hundreds of watts per metre per kelvin, the corresponding values for the elements of the middle part of the Mendeleev table being several watts per metre per kelvin, and that for the heavier elements occupying the lower part of the Table even to several tenths of a watt per metre per kelvin. A striking feature is that the lattice heat conductivity of crystals with light particles and rigid bonds may be very high. Thus at room
l at ti c e’ '» 8
Figure 4.9 Temperature dependence of heat conductivity of synthetic sapphire.
temperature la t tic e of diamond is greater than the total heat con ductivity of the best heat conductive metal, silver: SPAg = 407 W/(mK). At temperatures below the Debye temperature there is a sharp drop in phonon concentration with a fall in temperature leading to a sharp increase in their mean free path, so that at f ^ 0/20 it becomes comparable with the dimensions of the crystal. Since the crystal surface usually is a poor reflector of phonons, any further decrease in temperature does not lead to an increase in A,ph, for the latter is determined by the crystal’ s dimensions only. The tempera ture dependence of the lattice heat conductivity within this range of temperatures is determined by the temperature dependence of the heat capacity Cv . Since Cv CC Ts in the low temperature range, ^lattice too should be proportional to Tz: ^ la ttice o c r 3 (4.56) This result is also in qualitative agreement with experiment. Fi gure 4.9 shows the temperature dependence of thermal conductivity of synthetic sapphire. In the low temperature range la t t ic e is indeed approximately proportional to T3.
130
Solid State Physics
As the temperature rises so does the concentration of phonons nphr and this should per se cause la t t ic e to rise. However, an increase in nph is accompanied by an increase in the phononphonon scattering and a consequent decrease in the mean free path of phonons Xph, which should result in a decrease in SKlattice* For low nph the first factor should be the predominant one and l a t t i c e should rise with T. However, starting with a definite concentration wph the second factor should assume primary importance and l a t t i c e after passing through a maximum should fall with the rise in T . This decrease in the high temperature range is approximately of the 1IT type. Amorphous dielectrics in which the size of regions with a regular structure is of the order of interatomic distances should present a similar picture. Phonon scattering on the boundaries of such regions should be the dominant factor at all T's and therefore A,ph should be independent of T. Because of that the heat conductivity of such di electrics should be proportional to T 3 in the low temperature range and independent of T in the high temperature range. This is just what is observed in experiment. However, at present the theory is unable to predict not only the exact values of lattice heat conductivity, lattice? but even its order of magnitude. Heat conductivity of metals. In metals, in contrast to dielectrics, heat is transported not only by phonons but by electrons ^s well. Therefore generally the heat conductivity of metals is the sum of the lattice heat conductivity la t tic e (conductivity due to phonons) and the heat conductivity we obtain = 0
(5.5)
where U is the potential energy, E the total energy, and m the mass o f :the electron. For electrons sufficiently strongly bound to the atoms the poten tial energy may be written in the form U = Ua + 8U
(5.0)
where Ua is the electron’ s energy in an isolated atom. In a crystal it is a periodic function with a period equal to the lattice parameter, since there is a recurrence in the value of energy as the electron moves
U,
nrn
Figure 5.4 P e rio d ic varia tion o f electron p o te n tia l en ergy in crystal.
tfrotn one atom to another (Figure 5.4); 8Z7 represents a correction tfiatitakes account of the effect of neighbouring atoms on this energy. If one neglects the correction 8U in (5.6), that is, considers only the zero approximation, one should take the wave function and the energy EJji, I) of the electron in an isolated atom as the wave function and the energy of the electron in a crystal: ^ = \)a, E = = E a{n, Z), where n and Z are the principal and orbital quantum numbers, which determine the energy of the electron in an atom. In this case the difference between a crystal and an isolated atom is that in an isolated atom a specified energy level E J ji, Z) is unique, but in a crystal consisting of N atoms there are N Such levels (Figure 5.5). In other words, every energy level of an isolated atom is TVfold degenerate in a crystal. Such degeneracy is termed trans positional. . Now let us estimate the correction 8U in the potential energy (5.6). As the isolated atoms are brought together to form a lattice each atom increasingly feels the field of its neighbours with whom it inter acts. As we have already seen, such interaction results in the lifting of degeneracy including transpositional degeneracy. Because of that each level nondegenerate in an individual atom splits up into N closely ^spaced sublevels to form an energy band.
140
Solid State Physic*
If every level in an isolated atom was (2 1 + 1) times degenerate,, the corresponding band shall contain N (21 + 1) sublevels. Accordthe s level produces the s band consisting of N sublevels and capable of carrying 2N electrons; the p level produces the p band consisting of 3N sublevels and capable of carrying 6A electrons; etc. The separation between the sublevels in an energy band of an ordi nary crystal is very small. A crystal of a volume of one cubic metrecontains 1028 atoms. For a band of the order of 1 eV wide the sepa ration between the sublevels is about 10“28 eV. This separation is so Figure 5.5 E ach a to m ic en ergy le v e l E a in a sy stem con sistin g, o f TV a tom s is repeated TV tim es (is TVfold degenerate).
negligible that the band may be considered to be practically contin uous. However, the fact that the number of levels in a band is finite is very important for the determination of the distribution of electrons over states. The maximum effect of the lattice field is on the external valence electrons. Because of that the state of such electrons in a crystal experiences the greatest change and the energy bands formed by their energy levels are the widest. The internal electrons, which are strongly bound to their nuclei, are only slightly perturbed by the presence of neighbouring atoms and accordingly their energy bands in the crystal are almost as narrow as the levels of isolated atoms. Figure 5.6 shows a schematic diagram of energy band forma tion from discrete atomic levels. Thus in a crystal there is an allowed energy band to correspond to each energy level of an isolated atom: the 1s band to correspond to the 1s level, the 2p band to the 2p level, etc. The allowed energy bands are separated by forbidden energy bands E g. As the energy of an electron in an atom is increased so is the width of the respectiveenergy band, the width of the forbidden band being reduced. Figure 5.7 shows the energy band structure of lithium, beryllium, and elements having the diamond lattice (diamond, silicon, ger
141
The Band Theory of Solids
manium). In the lithium crystal (Fig. 5.7(a)) the splitting of the is level is a narrow one, the splitting of the 2s level being wider so that a sufficiently wide 2s energy band is formed. In the beryllium crystal V
where C is the wave’ s amplitude. As is well known, the square of the modulus of the wave function is proportional to the probability of detecting the electron in a specie Figure 5.8 Motion of a free electron: (a)—dependence of energy on wave vector (dispersion curve); (b)—square modulus of wave function proportional to the probability of the electron being at point x. E
C
2( c o s 2kx
+ sin 2kx) = C 2
*
0 (a)
( k )
fied region of space. As may be seen from (5.12), for a free electron} this probability is independent of the electron’ s^ position£since \) a
= C2
(5.13>
which means that for a free electron every point in space is equivalent and the probability of detecting it is everywhere the same (Figure 5.8(b)). The case of an electron moving in a periodic field of a crystal formed by regularly arranged ions is different (Figure 5.9). The proba bility of detecting it in a specified point of the crystal should be a periodic function in x , since positions displaced from one another by a multiple of the lattice constant a (for instance, the positions D, D \ and B in Figure 5.9) are equiprobable for the electron. The posi tions inside a period a (for example, inside D F D f) are, however, all different. This means that the amplitude of the wave function ^(x) of an electron moving in a periodic field does not, as in the case of a free electron, stay constant but changes periodically, or it may be said to be modulated with a period equal to the lattice parame ter a. Denote this amplitude u (x). Then the wave function of theelectron moving in a periodic field of a crystal in the direction of the x axis may be expressed in the following form: ip (x) = u (x) eihx
(5.14)
144
Solid State Physics
where u (x + no) = u (#), where n is an arbitrary integer. Relation (5.14) is termed the Bloch function. The specific form of this function is determined by the potential energy U (x), which enters into the Schrodinger equation (5.5). There should be a corresponding change in the dispersion relation for electrons moving inside a crystal as compared with that for free electrons. Firstly, as we have already seen, the energy spectrum of such electrons assumes a band pattern: allowed energy bands formed from corresponding atomic levels E a are separated by forbidden energy bands. Secondly, calculations show the electron energy inside each Figure 5.9 Motion of an electron in periodic field. The square modulus of the wave function that describes tne probability of the electron being at point x ofjthe horizontal axis is a periodic function •of coordinate x, the period being equal to the lattice parameter a.
hand to be a function of the wave vector k, which for a onedimen sional crystal (an atomic chain) with the parameter a is of the form E (k) = E a + C + 2A cos ka
(5.15)
where E a is the energy of the atomic level from which the band was formed; C is the displacement of this level due to the effect of the field of neighbouring atoms; A is the socalled exchange integral, which takes into account the newly created probability for an elec tron to move from one atom to another owing to the overlapping of the atomic wave functions (see Figure 5.3(b)). The exchange integral is the greater the greater the overlapping of the wave functions, that is, the greater is the exchange rate of the electrons of neigh bouring atoms. For s states A s 0, therefore it is reasonable to write out relation (5.15) individually for the s and the p bands. For the s bands E 8(k) = E's — 2A8c o s ka
(5.16)
E p (k) = Ep + 2 A P cos ka
(5.17)
and for the p bands
145
The Band Theory of Solids
where E's = E as + Cs, E ’ v = E ap + Cp, and A s and Ap are the ab solute values of the exchange integrals for the respective states. Figure 5.10 shows dispersion curves E (k) for the s and p bands drawn to satisfy equations (5.16) and (5.17). For the s states E s at k = 0 assumes its minimum value E s r,ln = E's — 2A s. As k increases, cos ka decreases and the value of E s (k) rises reaching its Figure 5.10 Dispersion curves for an electron moving in a periodic field: the lower curve corresponds to the s band, the upper curve to the p band; dotted lines are parabolas expressing the E(k) dependence in the centre and on the boundaries of the Brillouin zone.
Bi
< 3.
Ev
Z=W'
maximum E s max = E's + 2AS at k = n/a. In the interval of values of k from 0 to —jt/a, E s (k) changes in a similar fashion. The width of the allowed s band from E s mln to E s max is A2?a = Z?amax
E8m\n= AAs
(5.18)
As may be seen, it is determined by the absolute value of the exchange integral, which, in its turn, depends on the overlapping of wave func tions of neighbouring atoms. The shape of the curve E s (k) is that of an overturned bell. For the p states Ep mln = Ep — 2Ap corresponds to k = ± nla, and Ep max = Ep f 2Ap to k = 0. The width of the p band A £ p = £ p max
E p min — 4^4p
(5.19)
as in the previous case, is determined by the absolute value of the exchange integral Ap. As a rule, the higher the atomic level the greater the overlapping of the corresponding wave functions in the crystal, the greater the value of the exchange integral, and the wider the energy band formed from this level. For this reason high atomic levels are the origin of wide energy bands separated by narrow for bidden bands (see Figure 5.6).
146
Solid State Physics
The intervals of k inside which the electron energy E (k) as a period ic function of k completes its full cycle are termed Brillouin zones. For a onedimensional crystal (an atomic chain) the first Brillouin zone lies between k = —nla and k = jx/a and is 2n/a wide (Fig ure 5.10). In the vicinity of a dispersion curve’ s extremum, that is, in the vicinity of k = 0 and k = ±jc/a (the centre and the boundary of the first Brillouin zone), cos ka can be expanded into a power series in ka (k is measured from 0 if the extremum is in the centre of the Brillouin zone and from ±nla if it is on its boundary) leaving only two terms of the expansion cos ka = 1 — (ka)2/2 + . Substituting this into (5.16) and (5.17), we obtain E s (k) = E $wXn f+ A s (ka)2, E p (k) = Ep max — Ap (ka)2. The minimum of the dispersion curve E (k) is termed the bottom of the energy band and the maximum the top of the band. Therefore we may rewrite the sought for relations in a more general form: ^bottom (&) = ^min + A (ka)2
(5.20)
for the bottom of the band, and E i0V(k) = Emax~A'(ka)2
(5.21)
for the top of the band. Hence close to the top and the bottom of an energy band the por tion of the electron energy that depends on the wave vector is pro portional to the square of the wave vector, measured in the way indi cated above, and to the exchange integral that determines the width of the band. The parabolas corresponding to equations (5.20) and (5.21) are shown in Figure 5.10 by dotted lines. The E(k) dependence for real crystals is, as a rule, much more complex than that expressed by formula (5.15). Figure 5.11(a) shows the dispersion curves for the bottom of the conduction band (curve 1) and the top of the valence band (curve 2) of silicon. We see that the bottom of the conduction band, D , of silicon is not in the centre of the Brillouin zone but near its boundary in the direction [100]. The valence band is bounded by a curve in the shape of a parabola with its apex at B in the centre of the Brillouin zone. However, despite such complexity of the dispersion curves, the quadratic dependence of E (k) expressed by formulae (5.20) and (5.21) remains valid for both bandedges in this case. The width of the forbidden band, or energy gap, is determined by the minimum gap between the valence and the conduction bands; in Figure 5.11(a) this is denoted by E g. Frequently, when making a simplified analysis of the energyband structure of semiconductors, instead of the actual dispersion curves, which bound the valence and the conduction band, use is made of
147
The Band Theory of Solids
two parallel lines, one drawn tangentially to the bottom of the con duction band and the other to the top of the valence band (Fig ure 5.11(b)). The first line is taken to represent the lower boundary Figure 5.11 Band pattern of silicon: (a)—dispersion curves E(k) bounding the conduction band (curve 1) and the valence band (curve 2); the energy minimum of the conduction band is at point D in the [100] direction, energy maximum of the valence band is in the Brillouin zone centre B ; the distance between minimum D and maximum B is the forbidden band width E g\ (b)—schematic representation of energy band pattern of silicon. Conduction
(the bottom) of the conduction band and the second the upper bound ary (the top) of the valence band. The separation between the lines is equal to the forbidden band width E g.
§41 Effective mass of the electron The de Broglie formula establishes the following relation between the momentum of a free electron and its wave vector: p = hk
The velocity of the electron’ s translational motion is v = p/m = (him) k Differentiating (5.11) with respect to k, we obtain
(5.22)
148
Solid State Physics
Substituting this into (5.9) and (5.22) we obtain j 7
Ttl
dE
j
p = hk= j r n r '
1
dE
V= ^ k = — ^ F
/r
r\Q
\
Expressions for the momentum and for the velocity of translational motion written in this form turn out to be valid not only for free electrons but for electrons moving in a periodic crystal field as well. Momentum p is in the latter case termed quasimomentum of the elec tron. Set up an external field S in the crystal. This field acts on the elec tron with a force F = —qS imparting to it an acceleration . _ d u _ _ _j__d _ ( dE \ _ ^ dt Ti dt \ dk )
1
h
d2E dk dk2 dt
The work performed by the force F during the interval dt is dW = Fvdt = ^  ^  d t h dk
This work is spent on increasing the electron’ s energy by an amount dE = (Flh) (dE/dk) dt. Hence F/h = (dkldt). Substituting into the righthand side of the expression for /, we obtain F d2E _ 1 ~ h2 dk2
d2E _ h2 dk2 ~
q%
q% m eff
(5.24)
Formula (5.24) establishes the relation between the electron’ s acceleration j and the external force F with which an external field % acts on it. Hence it is an expression of Newton’ s second law. It fol lows then that the electron acted upon by an external force moves in a periodic crystal field on the average in the same way as a free elec tron would move if its mass were m° tt= h2l ( i ^ )
The mass metf is called the effective mass of the electron. Having attri buted to the electron in a periodic crystal field a mass me we may now regard it as being free and describe its motion in an external field in the same way as we would describe the motion of an ordinary free electron. However, the effective mass, which embraces all the details of electron motion in a periodic crystal field, is a very particular quan tity. To begin with, it may be positive or negative, many times larger or many times smaller in magnitude than the electron’ s rest mass m. Let us make a more detailed study of the problem.
149
The Band Theory of Solids
For electrons close to the bottom of a band the energy is ^bottom = = Emin + A (&a)2, the second derivative with respect to k being cPEIdk2 = 2.4a2. Substituting into (5.25), we obtain the following expression for the effective mass of the electron, which we shall de note mn: h2 (5.26) mn 2Aa2 Since A > 0, we see that mn > 0. Hence electrons close to the bottom of an energy band have a positive effective mass. For this reason they behave normally in an external field, accelerating in the direction of the acting force. The difference between such electrons and free electrons is that their mass may be quite different from the rest mass. It may be seen from (5.26) that the greater A is, that is, the wider the allowed band, the less the effective mass of the electrons occupying states close to the bottom of the band is. For electrons close to the top of the band the energy is E top = = S'max — A' (ka)2, the second derivative of E with respect to k being cPEIdk2, = —2A 'a2, and the effective mass, which we denote m’ nt is h2 (5.27) m'n = 2A'a2
It is a negative quantity. Such electrons behave abnormally in an external field set up in a crystal: they are accelerated in the direc tion opposite to the acting force. The absolute value is, as before, determined by the width of the energy band: mn is the smaller the wider the band is. Let us now find what is responsible for such a “ strange”behaviour of the electron in a crystal. In case of a free electron all the work W performed by an external force F is spent to increase the kinetic energy of the electron’ s trans lational motion: mv2 h2 W = Ek 2m Differentiating 2?k twice with respect to k, we obtain d2EJdk2= h2lm. Substituting into (5.25), we find that 7neff = m. Hence the effective mass of a free electron is simply its rest mass. The situation may be quite different in a crystal where the electron has not only kinetic energy but potential energy as well. When the electron moves under the action of an external force F, some of the work performed by this force may be transformed into kinetic ener gy 2?k, the rest being transformed into potential energy £/, and W = = + U In this case the result will be a smaller increase in kinet ic energy and, consequently, in electron velocity than in the case
150
Solid State Physics
of a free electron. The electron, figuratively speaking, gains weight and moves under the action of the force F with a smaller acceleration than a free electron would. Should the entire work of the external force be transformed into potential energy U, that is W = U, there would be no increase in the kinetic energy and in the velocity of the electron and it would behave as a particle of infinite effective mass. Finally, if in the course of the electron’ s motion not only the entire work of the external force F but some of the kinetic energy E £ that the electron had initially too shall be transformed'into the potential energy, so that U = W 4 E £, then as the electron moves along the crystal its velocity shall diminish, it shall be accelerated, behaving as a particle with a negative effective mass. Just such is the behaviour of electrons occupying states close to the top of the conduction band. However, a situation is possible in a crystal when in the course of the electron’ s motion under the action of an external force F not only the entire work of this force but some of the electron’ s poten tial energy, say U', shall be transformed into its kinetic energy so that 2?£ = W 4 U*, The E £ and the velocity v of such an electron Figure 5.12 fDependence of electron energy E , group velocity v, and effective electron mass mett on k. E
i meff
The Band Theory of Solids
151
shall rise quicker than those of a free electron. It looses weight as compared with the free electron, so that its effective mass met{ 0 K. Fifth electron
158
Solid State Physics
The remaining positive charge (a “ hole” ) is localized on the immobile arsenic atom and does not take part in electrical conductivity. The impurities which supply electrons are termed donors and the energy levels of those impurities donor levels. The semiconductors doped with donor impurities are termed ntype semiconductors. Acceptor levels. Let us suppose now that some of the germanium atoms in the germanium lattice are replaced by trivalent indium atoms (Figure 5.16(a)). The indium atom lacks one electron to estab lish bonds with all the four nearest neighbours. It can “ borrow”this Figure 5.16 Charge carrier excitation in a ptype semiconductor: (a)—atoms of trivalent indium in the germanium lattice at T = 0 K (the fourth bond of the indium atom is unpaired); (b)—at T > 0 K the electrons can go over to unpaired bonds of impurity atoms creating an indium ion and a vacant level (hole) in the valence band of germanium; (c) —energy levels of unpaired bonds of indium atoms are acceptor levels; (d)—electron transition from the valence band to an acceptor level at T > 0 K result in the generation of holes in this band.
Conduction band
1 Ec
A cceptor levels
oooooo(c) Conduction band
Fc rC^ Acceptor levels
6K >eeoe
73o “o 5 “
Valence band
(b)
(d)
K
The Band Theory of Solids
T59>
electron from a germanium atom. Calculations show that the neces sary energy is of the order of E a » 0.01 eV. The ruptured bond cor responds to a hole (Figure 5.16(b)) since it results in the formation of a vacant state in the valence band of germanium. Figure 5.16(c) shows the band pattern of germanium doped with indium. Directly above the valence band at a distance of E a » « 0.01 eV away from it there are some empty levels of the indium atoms. Those levels are so close to the valence band that already at relatively low temperatures some electrons from the valence band go over to the impurity levels (Figure 5.16(d)). They establish bonds with the indium atoms and loose their ability to move in the germa nium lattice playing no part in the conductivity. Only the holes created in the valence band act as charge carriers. The impurities that trap electrons from the valence band are termed acceptors and the energy levels of such impurities acceptor levels. The semiconductors doped with such impurities are termed ptype semiconductors.
§ 45 Position of the Fermi level and free carrier concentration in semiconductors Dependence of free carrier concentration on the position of the Fermi level. One of the main parameters of the gas of free carriers in a semiconductor is its chemical potential, p. As applied to the electron and hole gases the usual term for it is the Fermi level. As we have ascertained in Chapter 3, the Fermi level in metals is the last occupied level in the conduction band (see Figure 3.4): at absolute zero all levels below the Fermi level are occupied by elec trons and all levels above the Fermi level are empty. The concen tration of the electron gas in metals is comparable, as regards its order of magnitude, to the number of states in the conduction band; because of this the gas is degenerate and the distribution of the elec trons over the states is described by the FermiDirac quantum sta tistics. The electron concentration of such a gas is practically inde pendent of temperature. In the intrinsic and lowdoped impurity semiconductors the elec tron (the hole) gas is nondegenerate and the distribution of electrons over the states is described by the MaxwellBoltzmann classical statistics. For such semiconductors the free carrier concentration is dependent on the position of the Fermi level and on temperature. Let us find this dependence. Figure 5.17 shows the band pattern of a nondegenerate semicon ductor. At some temperature T other than absolute zero, there are some electrons in the conduction band of such a semiconductor and
Solid State Physics
160
some holes in its valence band. Denote their concentrations by n and p respectively. Take as the zero energy level the bottom of the conduction band. Choose a small energy interval dE lying between E and E + dE close to the bottom of the conduction band. Since the electron gas in a semiconductor is a nondegenerate gas, the num ber of electrons dn in the energy interval dE (per unit volume of semiconductor) may be calculated with the aid of (3.28): dn = ij (2mnf n e*lk*Te~m vT E l/2 dE
(5.29)
In nondegenerate semiconductors p is negative [see (3.48)]. This sraeans that the Fermi level in such semiconductors is below the
! .top Conducti on
band
\E + dF.
77777/ 7/ 7777//\f
L i i t i t t )E
Figure 5.17 Band pattern of a nondegenerate semiconductor: E c is the bottom of conduction band, Ey the top of valence band, jn .the Fermi level, and Eg the forbidden band width.
a O ooooooo £v Valence
band
'bottom of the conduction band, as shown in Figure 5.17. Denote the distance from the bottom of the conduction band to the Fermi level and from the Fermi level to the top of the valence band by p and p' respectively. Evidently p + p' = — Eg, or p' = — {Eg + p) (5.30) where Eg is the width of the forbidden band of the semiconductor. To obtain the total number of electrons in the conduction band at temperature T we integrate (5.29) over the energy values correspond ing to the conduction band, that is, from 0 to E Xov: Etov
„ = 4 n (  ^ ) 3/V /ABT [ eE/h*T E l/2dE o The function e~E/hBT decreases very rapidly as E grows; therefore it is permissible to substitute infinity for the upper limit to obtain n = 4n
j e~E/kBT E U2 dE o
161
The Band Theory of Solids
Evaluation of this integral yields n = 2 ( i g f f i p r j 3/2 en/ftBr
(5 .31)
A similar calculation carried out for holes generated in the valence band yields the expression p = 2(
) 3/2 e
= 2 ( 2nmj>**T.) 3/2 gt*V>Br
(5.32)
where is the effective mass of the hole. It follows from (5.31) and (5.32) that the concentration of free charge carriers in a band is determined by the distance from the boun dary of this band to the Fermi level: the greater this distance the smaller the carrier concentration (since (x C 0 and p' < 0). According to (5.31) and (5.32) the product of n and p for any nondegenerate semiconductor is np = 4
(mnmp f /2e~Eg/h&T
(5.33)
Formula (5.33) shows that for a definite temperature the product of the electron and hole concentrations is a constant for the respec tive semiconductor. This is an expression of the law of mass action as applied to the free carrier gas in semiconductors. Let us now discuss separately the position of the Fermi level and the free carrier concentration in intrinsic and impurity semiconduc tors. Position of Fermi level and carrier concentration in intrinsic semiconductors. In intrinsic semiconductors the concentration of electrons in the conduction band, n{, is equal to that of holes in the valence band, p {: ni = Pi (5.34) since every electron that goes over to the conduction band leaves behind a hole in the valence band. Equating righthand sides of (5.31) and (5.32), we obtain 2 ^ 2nmnkBT y/2 glx/ftRr = p ^ 2nmpkBT j 3/2c ~(Ea+\i)JknT
Solving this equation for p, we obtain
H =  T L+ T V ’1n ~
(535)
This relation determines the position of the Fermi level in intrin sic semiconductors. At absolute zero (T = 0) (i =
— Eg/2
(5.36)
162
Solid State Physics
that is, the position of the Fermi level is exactly the middle of the forbidden band (Figure 5.18). As the temperature rises the Fermi level shifts upwards towards the bottom of the conduction band if mp > mn, and downwards towards the top of the valence band it mv
_ q2n XpVp
(6.13v'> wJT TF _ yF where XF is the mean free path of the electrons with Fermi energy, Vy their velocity, and vF the number of collisions after which the directional velocity of such electrons becomes randomized. Figure 6.4 Mechanical model of the behaviour in an electric held of (a) a nondegenerate and (b) a degenerate electron gas; arrows denote the drift velocity in the electric held*
Here is a rough mechanical analogy to explain the different behav iour of a nondegenerate and a degenerate electron gas in an electric held. Imagine small charged balls (“ particles” ) floating on the surface of water in a flat horizontal vessel A and moving at random with different velocities in the absence of an external held (Figure 6.4(a)). Now let us place this vessel in an external held e, the wavelength X of the luminescent light should be longer than that of the light which initiates luminescence (X > X0) and this is what Stokes’law states. When the incident quantum collides with an excited atom, its energy e 0 = hv0 may be added to the excitation energy e causing the generation of a quantum with energy exceeding the energy of the one which initiates luminescence. This is the origin of antiStokes luminescence. V avilov’ s law. Consider the simplest case of every incident pho ton e 0 = hv0 generating a luminescent photon e = hv (quantum ef ficiency unity). Then the efficiency of the luminescence will evi dently be equal to the ratio of the energies of those photons: r\ = = e/e0. Since e = hv = hctX, it follows that n = v/v0 = XJX (6.51) From (6.51) we see that the luminescence efficiency should grow in proportion to the wavelength of the excitation, as required by V avilov’ s law. When X0 attains a value for which the energy of the incident quanta is not enough to initiate luminescence, the effi ciency drops abruptly to zero.
§62 Fundamentals of superconductivity Phenomenon of superconductivity. Investigating the role played by impurities in residual resistance, H. Kamerlingh Onnes in 1911 carried out experiments with ultrapure mercury. The results of those experiments were startling: at a temperature T ct = 4.2 K the spe cific resistance p of mercury fell to zero (Figure 6.26). This phenome non became known as superconductivity. The temperature T& at which the transition to the superconducting state takes place is termed critical, or transition, temperature. For thallium, tin and lead it is equal to 2.35 K, 3.73 K and 7.19 K, respectively (Figure 6.26). Since according to Ohm’ s law p = %!i, the condition p = 0 means that for a finite current density i the intensity of the electric field % at any point of the conductor is zero: & = 0. Experiments carried out at M.I.T. showed that a current of several hundred amperes once induced in a superconducting ring continued to flow without attenuation for a whole year.
208
Solid State Physics
Up to now over 20 pure chemical elements and several hundred alloys and chemical compounds have been found to be superconduc tive. They have transition temperatures ranging from 0.01 to 20 K. In 1933 W. Meissner and R. Ochsenfeld found that the phenomenon of superconductivity consists not only in ideal conductivity, that is, zero specific resistance. The magnetic field is pushed out of the bulk of a superconductor no matter how this field was established— by an external magnet or by a current flowing in the superconductor itself. This means that the magnetic induction B t inside the super conductor is always zero as long as it/ is in the superconducting state. Figure 6.26 Abrupt change in specific resistance of mercury, tin,jlead and thallium in the course of transition to superconducting state. p, K)'* ohmm
In other words, the superconductor is an ideal diamagnetic whose magnetic susceptibility % = —1. It will be shown in the following chapter that normal diamagnetics have % 1. Hence superconductivity is a combination of two simultaneous phenomena—that of ideal conductivity and of ideal diamagnetism. The superconductive state can be destroyed by a magnetic field. The necessary magnetic field H cr is termed critical. The value of H CT depends on the temperature: at T = T ct the critical field intensity is zero. With the decrease in temperature H cr rises and is maximal at absolute zero. The temperature dependence of H CT for lead and tin is shown in Figure 6.27. Fundamentals of theory of superconductivity. Despite the fact that over 60 years have gone by since superconductivity was first discovered, the microscopic theory of this phenomenon is a quite recent development due mainly to Bardeen, Cooper, Schrieffer. The abbreviation for it is the BCS theory. Let us discuss this theory in general terms. Gap in the energy spectrum of conduction electrons in a supercon ductor. We again recall the causes of a finite electrical resistance of normal conductors, for instance, of metals in a normal state. If we neglect the periodic nature of the m etal’ s lattice potential (the Som
209
Electrical Conductivity of Solids
merfeld model), we can regard it as a potential trough for the electrons, having a flat bottom and filled by electrons up to the Fermi level E F (see Figure 3.4). The kinetic energy of such electrons is given by (5.11) F_
p2 _ n 2k2
2m
2/7i
Figure 6.28(a) shows once again the E versus k dependence corres ponding to (5.11): thin horizontal lines denote the occupied levels, the solid line denotes the Fermi level EF, and kF and —kF are wave vectors corresponding to this level. Figure 6.27 Temperature dependence of critical field intensity H cr in superconductor.
Figure 6.28 Dependence of free electron energy in conduction band of a metal on wave vector: (a)—in the absence of external field; (b)—external field its effect is to excite precession of the orbit around the direction of the field (Figure 7.11(b)): the perpendicular pt to the plane of the orbit describes a cone around H. Calculations show that the angular velocity of such a precession is expressed by formula (7.37). Induced magnetic moment of an atom. Magnetic susceptibility of diamagnetics. The precession of the electron orbit results in an additional motion of the electron around field H. This motion is superimposed on its orbital motion. The magnetic action of this additional motion is equivalent to that of a closed current A , (7.38) where vl is the precession frequency related to the angular frequency by the expression col = 2kvl . The minus appears because of the negative charge of the electron. The magnetic moment of the elementary current AI is 4^ = 4 I S =  £ L
b,
(7.39,
where S is the area bounded by the path of the electron precessing around field H. Calculations show that S = 2jir2/3, where r2 is the mean square of the electron’ s distance from the nucleus. There fore q*r2 q2r 2 Ai = \i0H (7.40) 6m B0= 6m It follows from formula (7.40) that in a magnetic field every elect ron acquires an additional socalled induced magnetic moment direct ed against //. The appearance of this moment is the cause of the
Solid State Physics
240
magnetization of the body in the direction opposite to that of the magnetic field, which is characteristic of diamagnetics. The magnetic moment of an atom containing Z electrons is found by adding up the moments of individual electrons: z
AM= S Si F?
where r2 is the mean square distance of the ith electron from the nucleus. The sum of r\ may be replaced by the product Za2, where a2 is the mean square distance of all the electrons from the nucleus. Then Za2q2 D
AM =
‘ “6^*
(7.42)
o
Multiplying (7.42) by the number of atoms per unit volume, n, we obtain the magnetization J m: Zq2na2 D _
J w = nAM =
Zq2na2
1
6m
H0H
(7.43)
The magnetic susceptibility is X= ^
H
=
6m
(7.44) v
'
Assuming that a « 10~10 m and n & 5 X 10~28 m~3, we obtain 10” 6Z. This is in good agreement with the data of Table 7.1. Moreover, from (7.44) it follows that magnetic susceptibility of diamagnetics is independent both of temperature and of magnetic field intensity H and rises in proportion to the atomic number of the element, Z, which is in full agreement with experiment.
§67 Origin of paramagnetism Langevin’ s classical theory of paramagnetism. The classical theory of paramagnetism developed by Paul Langevin is based on the idea that the atoms of paramagnetic materials have a permanent magnetic moment M, that is, they constitute permanent magnetic dipoles and that the interaction between these dipoles is negligible. The energy of such a dipole in a magnetic field H is Um = — Mno/7cos0
(7.45)
where 0 is the angle between M and H (Figure 7.12(a)), The minimum of Um corresponds to 0 = 0. Therefore all the dipoles tend to orient themselves in the direction of the external
241
M agnetic Properties of Solids
field, this being hampered by thermal motion. The total magnetic moment of the material is made up of the projections of the magnetic moments of the individual atoms on the direction of H. Since the magnitude of those projections is MH = M cos 0, the problem of the quantitative calculation of the magnetization of the material is reduced to the calculation of the average value of M H that corre sponds to the state of equilibrium between the orientational effect of the field and the disorientational effect of thermal motion. Just Figure 7.12 Explaining classical theory of paramagnetism: (a)—magnetic moment M and its projection MH on magnetic field H; (b)—calculating total magnetic moment of a paramagnetic; (c)—plot of the Langevin function.
H
this problem was solved by Langevin with the aid of methods of clas sical statistics. He supposed that the orientation of M with respect to H can be arbitrary and that accordingly the angle 0 can assume all values. The probability for a dipole to align itself at an angle in the interval (0, 0 + d0) to H (that is inside the solid angle see Fig ure 7.12(b)) is determined by the Boltzmann distribution function: W = C1e~Vto,hBTdSi = C i exp (u° M^
os6) dQ
where 6\ is a normalization constant. It may be seen from Figure 7.12(b) that dQ = 4ji sin 0 d0; there fore
ty = C ex p ( ^ where C is a new constant.
rcos9) Sin9d9
242
Solid State Physics
The average value of M n is n
J cos 0 exp
c o s
Q/kBT) sin 0 dQ
M H = M c o s Q = M ±  l i 
(7.46)
J exp (ii0MH cos Q/kBT) sin 0 dQ
o
If those integrals are evaluated, the result is j) = M ( c o th P where
a
P
j)
__ M \i0H
(7.47)
(7.48)
kBT
The magnetization is / m = nMH = nM ^ coth p — j j
(7.49)
where n is the number of atoms per unit volume, and the magnetic susceptibility is X = ^L= ^  (cothp — y )
(7.50)
Since the atomic dipoles acted upon by a field align themselves in its direction, such will be the direction of the magnetization of the body as a whole, which is characteristic of paramagnetics. Let us expand coth p in a power series: coth p = P1 f p/3 — — p2/45 + .... For p 1 we can limit ourselves with the first two terms of the expansion. Then nM$ _ nM2 rj ~ F “’ S k ^T ^0" '
A
\i0nM2 ^ = 3kBT
(751)
In full agreement with experiment Jm is directly proportional to H and inversely proportional to T. The second of the formulae (7.51) expresses the Curie law: % = C/T. The Curie constant C = = nM2\i0/(3kB). For atoms M « \iB; then for H « 106 A/m we see that MH\i0 « « 10~23 J and for T = 300 K we see that kBT » 3 X 10~21 J. Hence the condition p 1 is almost always satisfied. Only in very strong fields and at very low temperatures is p 1 and the direct proportionality between Jm and H is no longer maintained. In the limiting process, as p >■oo, coth p~> 1 and the magnetization becomes saturated, the corresponding maximum value being / s = nM
(7.52)
243
M agnetic Properties of Solids
Magnetic saturation involves the alignment of magnetic moments of all atoms in the direction of the field. The function L (P) = coth p — 1/p is termed the Langevin junc tion. Its plot is shown in Figure 7.12(c). For small P’ s a good approx imation for the plot is the segment of the straight line OA; as p oo the function L(P) 1. Fundamentals of quantum theory of paramagnetism. The classical theory is incapable of providing a consistent explanation of the magnetic phenomena as the result of the motion of electric charges. The existence of molecular currents necessarily involves the acknowl edgment of the fact of the stability of electronic motion in atoms, a fact unacceptable for classical physics. The assumption that all orientations of magnetic moments with respect to H are possible, which is the basis of Langevin’ s classical theory, is also wrong. Those difficulties have, on the whole, been overcome by the quantum theory s consider briefly the essence of this theory. of paramagnetism. L et’ There are 2J + 1 ways in which the atomic magnetic moment M j may align itself in a magnetic field (J is the intrinsic quantum number). The probability of each such orientation is determined by the Boltzmann distribution W = (M JH is the projection of M j on H). The average value of M JH will be* ■y I P0M j h H \ 2 j MJH exp [ k^ T j (7.53> Vi {NMjhH \ Z exP \  k ^  ) J The difference between (7.53) and the classical expression (7.46) is that integration is replaced by summation over the discrete direc tions in which the vector M j may be aligned. Evaluation !of the sums in (7.53) yields the following result:
__
where
M j H — g J Mn B j
(P)
(7.54)
R_ / g p B ^ o
p
(7.55)
kBT
B j (P) = ^
coth
P — £r coth ~2J
(7.56)
Function B j (P) is termed the Brillouin function. The magnetization and the magnetic susceptibility are equal to Jm = M JHn = ngJ\iBBj(f>) %= 16*
P)
(7.57) (7.58)
244
Solid State Physics
For p < 1, jBj(P) « P(/ + l)/(3J) and T n g ^ J (J+i) fXo/7 Jm ~ 3kBT '
______ (• /■ 41) M'bH'O 3kBT
tn (
coth ^  * l,
and the magnetization attains the saturation value Js = ngJ\iB
(7.60)
Materials used for experimental tests of the theory of paramagne tism are the solutions and crystalline hydrates of salts, which con tain ions with nonzero magnetic moment. Such are, for instance, the Figure 7.13 Calculating paramagnetism of free electrons.
(a)
(b)
(C)
ions of the elements of the groups of iron and rare earths. In solutions and in crystalline hydrates the ions are so far apart that their interaction may be neglected, which is a necessary condition for paramagnetism. Experimental investigations of such compounds have produced results in good agreement with the theory. Paramagnetism of electron gas. According to (7.51) and (7.59), paramagnetic susceptibility is inversely proportional to temperature. However, some metals have been discovered to exhibit paramag netism independent of temperature. It was Wolfgang Pauli who demonstrated that this is due to the paramagnetism of free electrons that constitute the electron gas. Figure 7.13(a) shows the conduction band of a metal. It is schemat ically represented in the form of two halfbands containing electrons with opposite spin moments \is = ulb When H = 0, the number of electrons in both halfbands is equal and the total magnetic moment
245
M agnetic Properties of Solids
of the electron gas is zero. When the field H is applied, every electron of the left halfband acquires an additional energy U'm = — poM'B# and every electron of the right halfband an energy U” m = x0iBH. The result is the appearance of a difference between the quasiFermi levels E F — E f = 2[i0pB# (Figure 7.13(b)) for the electrons of the right and the left halfbands which is equalized by means of spinflip of some of the electrons of the right halfband and their transi tion to the left halfband (Figure 7.13(c)). Since all the internal levels in the halfbands are occupied, the only electrons whose spins can be reversed are those occupying levels in the zone where the Fermi distribution is fuzzy (see Figure 5.6(b)) and where there are vacant levels. The number of such electrons, according to (3.43)), is (7.61)
where n is the electron gas concentration. Of this number An' = C exp (lio^b#/&b^) electrons will have their magnetic moments oriented in the direction of H and An" = = C exp (—(lio^b^/AbT1) against H (C is a constant). The magnetic moment per unit volume of a metal due to spinflip is J me = (An' — An") p,B = C>B (ep — e“p) where P = \jLQ\iBHtkBT Since An = An' f An" = C (e$ + e~V), it follows that C = = An (e$ + ^“ P)1. Substituting this into the expression for / me, we find J me =
p =
For P < 1, tanh P ^ P and An from (7.61), we obtain
tan h p
J me = An\i%\\0H/kBT. Substituting
J met t n ^ i i 0H
(7.62)
The paramagnetic susceptibility of the electron gas is (7.63)
X e ~ n Ef A more accurate calculation yields E j?
(7.64)
It may be seen from (7.64) that the magnetic susceptibility of the electron gas should be independent of temperature, which is what is observed in practice.
246
Solid State Physics
Production of low temperatures using the method of adiabatic demagnetization of paramagnetic samples. The atoms of paramagnet ic materials possess a permanent magnetic moment. In the absence of an external field as a result of thermal motion of the atoms the orientation of their magnetic moments is almost completely random. The quantitative measure of this disorder is the entropy S , which in this case is termed magnetic entropy S m. In compliance with the Boltzmann principle S M = kBln Wm (7.65) where Wm is the thermodynamic probability, which in this case is equal to the number of ways the n atoms of the paramagnetic sample can be distributed among the 2/ + 1 sublevels into which every atomic level splits in a magnetic field. Its value may be obtai ned from the expression Wu = {2J + \ r Substituting (7.66) into (7.65) we obtain S u = kBn In (2J + 1)
(7.66) (7.67)
When the magnetic field is applied and its intensity increased, an ever increasing number of magnetic moments is oriented in the direction of the field, the result being a reduction in the magnetic entropy. When the state of magnetic saturation is reached, the grea test possible order in the arrangement of magnetic moments is established and S M vanishes. Hence the process of magnetization of a paramagnetic sample up to saturation is accompanied by the decrease in its entropy by the amount AS = S m = kBn In (2J + 1) (7.68) If the magnetization is performed at a constant temperature T7, the decrease in S by the amount AS results in the generation of an amount of heat equal to AQ = TAS. This heat is transmitted from the sample to the surroundings, usually to liquid helium. After equilibrium has been established the helium is removed and the sample is left thermally insulated. In such conditions it is slowly adiabatically demagnetized with the result that its entropy again rises by AS. The rise in entropy requires heat, which can be supplied only by the thermal vibrations of the lattice since the sample is thermally insulated from the surroundings. Because of that its tem perature drops. Using this method it was possible to obtain tempera tures below 0.001 K. The possibility of obtaining still lower tempera tures is limited mainly by the fact that already at H = 0 the atomic energy levels are to some extent split into sublevels because of the interaction of the magnetic moments with each other and with the nucleus.
Magnetic Properties of Solids
247
§68 Origin of ferromagnetism Elementary carriers of ferromagnetism. A magnetized body acquires a magnetic moment M made up of regularly oriented atomic magnet ic moments and' an angular momentum P made up of regularly oriented atomic angular momenta. According to (7.17) and (7.26) the ratio MIP must be equal to q!2m if the magnetization is due to orbital magnetic moments of the atoms and to qlm if it is due to spin moments. The appearance of a magnetic moment in the course of magnetiza tion was first established in experiments of A. Einstein and W. J. Figure 7.14 Experiments on the nature of ferromagnetism: (a)—the experiment of Einstein and de Haas; (b)—experiment of Barnett; (c)—experiment of Ioffe and Kapitza.
de Haas and became known as the Einsteinde Haas effect. In those experiments a small iron rod 1 suspended on a thin elastic thread 2 was placed inside a solenoid 3 (Figure 7.14(a)). In the course of magnetization the rod turned and twisted the thread. The direction of rotation of the rod changed with the change in the direction of magnetization. The angle of rotation was measured with the aid of mirror 4 fixed on the rod which reflected a beam of light on scale 5. The experiment made it possible to determine M and P and to find the gyromagnetic ratio y = MIP. S. J. Barnett made an experiment which was the reverse of the Einsteinde Haas experiment: he observed the magnetization of a quickly rotating iron rod. Such magnetization is caused by the tendency of electrons—thought of as tops possessing angular mo
248
Solid State Physics
menta—to arrange their axes of rotation (spins) in the direction of the rotation axis of the body (Figure 7.14(b)). In another experiment the Soviet physicists A. F. Ioffe and P. L. Kapitza quickly heated a magnetized rod to a temperature above the Curie point. Before heating the orientation of the “ electron tops”was ordered (Fig. 7.14(c)) and their total angular momentum was nonzero. When heated to a temperature above the Curie point the “ tops” changed their orientation to chaotic (Figure 7.14(d)) and their total angular momen tum became zero. Because of that the demagnetized rod as a whole acquired a rotational momentum that could be measured in the experiment. Measuring in addition the magnetic moment of the magnetized rod one could find the gyromagnetic ratio y = MIP. The experiments demonstrated that the gyromagnetic ratio for ferromagnetic materials is MIP — — qlm, that is, equal to the gyromagnetic ratio for the intrinsic moments of the electron. This proved that ferromagnetism is due not to orbital but to spin magnetic moments of electrons, which is consistent with the electronic structu re of the atoms of elements that exhibit ferromagnetism. Since the magnetic moments of closed shells are zero and since the outer valen ce electrons are collectivized in the process of formation of the metal lic state, ferromagnetism must be a property solely of the transitio nal elements, which have incomplete inner shells. Those elements include the transitional metals of the iron group, which have an imcomplete 3d shell, and rare earth elements with an incomplete 4/ shell. Since, on the other hand, the orbital magnetic moments of the electrons of the 3d shell are “ frozen in”and their contribution to the magnetic properties is negligible, ferromagnetism of the elements belonging to those groups can be due only to the atomic spin moments, which in this case are quite large (Table 7.2). This hypothesis was first expressed by the Russian scientist B. Rozing in 1892 and was exploited later by the French physicist Pierre Weiss. The latter assumed that there is an intense molecular field H in a ferromagnetic proportional to the saturation magnetization J s: H = XJ8
(7.69)
where X is termed the molecular field constant. This field is responsible for the spontaneous magnetization of a ferromagnetic. The introduction of a molecular field made it possible to explain a wide range of phenomena observed in ferromagnetism. However, the nature of the field itself remained a mystery for a long time. At first it was supposed that the origin of forces which orient the spin moments is purely magnetic, that they appear as a result of an ordinary interaction of spin magnetic moments (spinspin interaction). The energy of this interaction is of the order of t/m ~ xB/a3, where a is the interatomic distance in the lattice of the ferromagnetic. Substituting p,B = 9.27 X 10~24 Am2 and a « 10“10 m, we obtain
(249
Magnetic Properties of Solids
Um » 10“23 J. This is about two^ orders of magnitude less than the room temperature thermal energy of a lattice atom which disturbs the orderly spin arrangement. It follows then that the magnetic spin interaction is incapable of effecting their parallel orientation characteristic of the ferromagnetics at temperatures below the Curie point and that the origin of the molecular field which effects such parallel spin orientation should be nonmagnetic. Subsequently this conclusion was proved by direct experiments of Ya. Dorfman. The role of exchange interaction in ferromagnetism. In 1928 Frenkel made the assumption that the origin of the forces which are respon sible for the definite mutual orientation of atomic magnetic moments is electrostatic. They are the result of exchange interaction of the electrons of inner incomplete atomic shells. We have already discussed this type of interaction in dealing with the nature of the covalent bond (see Section 3). The exchange interaction involves a change in the energy of the system. This is easily seen from the example of the simplest system of two hydrogen atoms (see Figure 1.5). According to (1.11) and (1.12) the energy of such a system is U = 2Eo+ % 0 2
(7.70)
w hereto is the energy of two noninteracting hydrogen atoms, ifyis the energy of Coulomb interaction of electric charges making up the atoms, S is the overlap integral whose value lies in the range 0 ^ 5 ^ 1 , and A is the exchange energy (in Chapter 5 we called it the exchange integral). Calculation shows that A can be expressed by the following relation (7.71) where S* and S7 are the total spins of the interacting atoms, and J is the exchange integral (it is a measure of the probability of electron 1 going over to atom B and of electron 2 going over to atom A), In the case of two interacting hydrogen atoms A =  J ( 3 r Sj)
J = j
1)50(1> ^ (2>
(2) *6 (!) d v i dV> (7.72) Here q2lr and q2/r12 are the interaction energies of the nuclei between themselves and of the electrons between themselves, respectively; —Q2/rbi and —g2/ra2 are the energies of attraction of electron 1 to nucleus b and of electron 2 to nucleus a; \;a(l) and x)b(2) are the wave functions that describe the motion of electrons 1 and 2 around nuclei a and fo, respectively; \)a(2) and ^ ( l) are the wave functions that describe the probabilities for electrons 2 and 1 to he close to nuclei a and b, respectively, that is, the probabilities of the atoms A and B exchanging electrons; and d,V1 and dV2 are volume ele ments.
250
Solid Stafe Physics
It follows from (7.72) that both positive and negative terms enter the exchange integral. Therefore the sign of the exchange integral may be either positive or negative. This is determined by the part played by the positive and negative terms of the exchange integral, which in its turn depends on the relation of the dimensions of the electron shells taking part in the formation of the exchange bond and on the interatomic distance. The sign of the exchange integral determines what orientation of the spins of electrons taking part in the exchange bond is advantaFigure 7.15 Spontaneous magnetization of a ferromagnetic. Exchange forces cause parallel orientation of the spins of electrons belonging to inner partially filled shells.
geous—the parallel or the antiparallel. It follows from (7.71) that when the sign of the exchange integral is negative (J 0), the exchange energy A will be negative and the energy of the system as a whole will be less than the energy of the individual atoms if the spins S, and S; of the electrons taking part in the exchange bond are parallel: S*  Sj Hence the parallel orientation of the spins of neighbouring atoms may too be advantageous from the energy point of view if their exchange integral is negative. This is the necessary condition for ferromagnetism since the parallel arrangement of spins and, conse quently, of spin magnetic moments results in spontaneous magneti zation, which is characteristic of ferromagnetics (see Figure 7.15).
Magnetic Properties of Solids
251
Figure 7.16 shows the dependence of the exchange integral J on the ratio of the lattice constant a to the diameter d of the 3d shell of atoms of the iron group transition metals. It may be seen from Figure 7.16 that at aid > 1.5 the exchange integral is positive; at aid < 1 .5 it turns negative, its absolute value increasing with the decrease in a!d. It follows then that of all the transition metals only iron, cobalt, and nickel should be ferromagnetic, which is indeed the case. Manganese and other elements of the group, for which a!d E x, it follows that n2 < and because of that reso nance absorption exceeds stimulated radiation and the system absorbs incident electromagnetic energy eventually transforming it into heat. For stimulated radiation to exceed resonance absorption the ther mal equilibrium of the system must be disrupted by raising the population of the higher levels above that of the lower levels, that is, to make n2 > nx. Such population is termed population inversion. Figure 7.26
Level population at various temperatures.
■oooooooooo
r= o k
—CHOOOOO—
T< OK
T > 0K
Quantum states with population inversion may conveniently be described with the aid of the concept of negative absolute temperature. From (7.78) we have £2~£i (7.79) &B ln (n2/nl)
In equilibrium n2 E 2 — E 1 > 0, and T > 0. In case of population inversion n2 > E 2 — E x > 0, and consequently T < 0 . Figure 7.26 shows the occupancy of states at various tempera tures. At T = 0 K all the particles occupy the lowest level 12 and the system ’ s energy is at its minimum (Emin = nE^. As the tempera ture rises some of the particles go over to the higher level and the energy of the system increases. At T = oo the population of the levels is equilized and the system ’ s energy reaches the maximum value it can have in equilibrium [^max = n {Ex + E 2)!2\. At T < 0 K the population of the higher level exceeds that of the lower level and because of that the energy of the systems turns out to be greater than Z?max. Hence the energy region corresponding to negative temperatures lies not below the absolute zero, as would appear at the first glance, but above infinite temperature. Should such a system be brought in contact with a body whose temperature is positive, the heat would be transported from the system to the body until a state of thermal equilibrium would be reached. It should be pointed out that negative temperature is a purely quantum effect and may be observed only in systems with a limited set of levels. 12 To avoid contradiction with the Pauli exclusion principle E1 and E 2 must be taken to mean narrow energy bands: from Ex to Ex f dE and from E 2 to E 2 dE.
Magnetic Properties of Solids
261
One may realize the population inversion in practice, for instance, by quickly reversing the direction of a constant magnetic field so that the time of reversal would be less than the relaxation time. With the field H 0 in the initial direction the population of the lower level is greater than that of the upper one; when the field is reversed Figure 7.27 Population inversion in a twolevel quantum system.
quickly the initial population of the levels remains unchanged but with respect to the new field H 0 direction it will be populated in versely (Figure 7.27). Principles of operation of masers. Suppose that an external signal with the resonant frequency co = (E 2 — E x)!h is applied to a twolevel system with a population inversion. This signal will induce Figure 7.28 Excitation of paramagnetic amplifier (a) and radiation of amplified signal (b).
the transitions of the particles: E 2> Ex and E 1+ E 2. Since in the case of population inversion the number of particles on the higher level exceeds that on the lower level and since the transition pro babilities w12 and w21 are equal, the stimulated radiation E 2> E x will exceed resonance absorption E x> E 2 and the signal will be amplified. Therefore such a system will do the job of an amplifier of electromagnetic radiation. The term for it is paramagnetic ampli fier (usually maser).
262
Solid State Physics
In practice not twolevel but threelevel quantum systems are used for paramagnetic amplifiers. The active materials in them are diamagnetically diluted crystals of paramagnetic salts; in wide use are ruby crystals (A120 3) doped with chromium and germanium ions. Figure 7.28(a) shows a quantum system with three levels: E±, E 2, E 3. The dotted line represents the dependence of the number of particles n on the energy E in thermal equilibrium. Such a system is placed in a magnetic field H 0 and irradiated with highfrequency electromagnetic radiation with a frequency co13 = (E3 — Ex)lh. This process is termed pumping. In pumping fields of high intensity (Figure 7.28(b)) saturation is achieved, when the numbers of particles on the levels E x and E 3 are equal (n3 = nx) and less than that on the level E 2: nx < l n 2, n3 < r a 2. Should a signal with a frequency co2i = = (E 2 — EJ/h be applied to such a system, it would be amplified by the stimulated transitions of the particles from the level E 2 to the level E x. The system will work as an amplifier. For a high amplification factor the difference in the population of the levels must be as great as possible. The way to do it is to cool the system to liquid helium temperatures. The concentration of the magnetic atoms should be low to exclude interaction of magnetic moments, which results in the widening of the absorption line and in the decrease in the amplification factor. One solution is to use diamagnetically diluted crystals of paramagnetic salts, of which the ruby crystal doped with chromium or germanium ions may serve as an example. The main advantage of the paramagnetic microwave frequency amplifiers is their ability to work at very low temperatures and, consequently, at low noise levels. This makes it possible to receive signals too weak for amplifiers of conventional types. The frequency tuning of the amplifier is done by changing the intensity of the field H q which in its turn changes the resonance absorption frequen cyPrinciples of operation of quantum generators. To devise a laser on the basis of the negative temperature quantum system a positive feedback should be provided to make sustained oscillations possible. To this end the system is placed inside a cavity with reflecting walls. In conditions in which each spontaneously generated quantum /xco stimulates the generation of, on the average, more than one quantum, the amplitude of the electromagnetic oscillations of the appropriate frequency co will grow continuously. The system will become selfexcited. The radiative energy contained in the cavity is removed via a wave guide. Such cavities are termed cavity resonators. They are constructed from highly conductive materials and their dimensions are close to the wavelength radiated by the laser. The feedback signal in provided by radiation reflected by the cavity walls, a careful choice of the dimensions and shape of the resonator being necessary
Magnetic Properties of Solids
263
to obtain the right phase relationship (the reflected radiation must be in phase with the generated one at the point of generation). The first quantum generators were designed by N. G. Basov and A. M. Prokhorov. They used twolevel oscillators and the generator operated on beams of ammonia molecules. The ammonia molecule NH3 is made up of three hydrogen atoms arranged in the base of a triangular pyramid and a nitrogen atom in the pyramid’ s vertex Figure 7.29 Ammonia molecule (a) and its energy levels (b).
(Figure 7.29(a)). This is the ground state of the molecule Ex. The molecule has an excited state E 2 (Figure 7.29(b)) in which the nitro gen atom is forced into the base plane. The normal NH 3 molecule is asymmetric and by force of this has a nonzero dipole moment. The dipole moment of an excited molecule because of its symmetry is zero. This fact makes it possible to separate the normal and excited molecules by passing the molecular beam through a nonuniform electric field. Such a field deflects normal polar molecules; the excited nonpolar molecules are not deflected. Figure 7.30(a) represents a schematic view of a molecular generator. It is made up of three parts: the beam source A , the separation system B, and the cavity resonator C. The source of the molecular beam is a small space 1 closed on one side by a fine mesh 2. A gas pressure of one mm Hg is maintained inside the space. The mqlecules forming the beam pass through the mesh into a vacuum chamber practically without collisions. A quadrupole condenser B (Figure 7.30(b)) is placed in the way of the beam setting up a nonuniform field (Figure 7.30(c)) that sorts out the molecules. The excited molecules (on the higher level) are con centrated close to the condenser axis and the normal molecules are deflected to the walls. In this way the beam close to the condenser
264
Solid State Physics
axis is made to contain mainly the excited molecules and thus a quantum system with population inversion, or with negative tempe rature, is created. From the separator B the molecular beam enters the resonator C turned to the frequency of the radiative transitions from the upper to the lower level [to the frequency o> = (E2 — E x)lh\ and induces in it electromagnetic oscillations with this frequency. The electro magnetic energy is transported via the wave guide 5. The molecules Figure 7.30 Schematic representation of a quantum generator operating on a beam of ammonia molecules: (a)layout of amplifier (A is the source of beam of ammonia molecules, B the separation system, C the cavity resonator); (b)—quadrupole condenser of separating system; (c) electric field in condenser. Output signal
in the beam practically do not interact and because of that the spec tral line of the oscillations is very narrow (1 kHz at v = 24 MHz). Another advantage of the molecular generator is its longterm fre quency stability. The oscillation frequency is determined solely by the structure of the ammonia molecule (that is, by E 2 — E ± ) and is therefore independent of other generator circuit parameters. This made it possible to use the ammonia oscillator as a frequency stan dard. The error of a clock using such a frequency standard for its “ pendulum”does not exceed one second in 300 years of continuous operation. In recent years quantum generators for the infrared and the optical spectral intervals (lasers) have been developed. Their use opens up wide possibilities for the development of communication, in loca tors, etc. For instance, an optical communication channel would be capable of carrying up to 10 000 TV programmes. Quantum gen erators nowadays are widely used for the machining of tough mate rials, in medicine, and in other fields of science and technology.
8
Contact Phenomena
§73 Work function The work function concept. The positive ions that make up the metal lattice establish in it an electric field with a positive potential that changes periodically along a straight line passing through the lattice sites (Figure 8.1(a)). As a rough approximation, this variation may be neglected and the potential be considered constant and equal to
Figure 8.1 Metal as a potential through: (a)—internal potential of metal; (b)—potential energy of electron in metal
V0 at every point of the metal. A free electron has a negative poten tial energy U0= — qV0 in this field (q is the electron charge). Figure 8.1(b) depicts the change in the potential energy of the electron as it passes from the vacuum into the metal: in vacuum U = = 0, in the metal U = U0 = —qV0. Although such a change has the nature of a jump, it takes place over a distance 8 equal approx imately to the lattice parameter. It may be seen from Figure 8.1(b) that the metal is a potential trough for the electron and that work should be performed to get the electron out of it. This work is termed the work function. 265
266
Solid State Physics
Should the electrons have no kinetic energy, the work needed to liberate them would be equal to the depth of the potential trough t/0. However, electrons possess kinetic energy of translational motion even at absolute zero since they occupy all the lower energy levels of the potential trough up to the Fermi level p. Therefore the energy needed to make them leave the metal is less than £/0. The least work must be performed to liberate the electrons occupying levels close to the Fermi level. It is equal to the separation % of the Fermi level from the zero level and the term for it is thermodynamic work function. The problem of estimating the electron work function of a semicon ductor is somewhat more complicated. As may be seen from Figure 8.2 Figure 8.2 Electron work function of semiconductor.
the electrons may leave the semiconductor from the levels of the conduction band at the expense of work from the impurity levels at the expense of work %l7 and from the levels of the valence band at the expense of work %2 and %3. The least work Xo is required to liberate the electrons from the conduction band. However, emission of only the conduction electrons would upset the equilibrium of the electron gas to reestablish which the electrons should go over to the conduction band from the impurity levels and from the valence band. Such tran sitions require work to be performed and in adiabatic conditions this work is performed at the expense of the internal energy of the crys tal, that is, as the state of thermal equilibrium is restored the crys tal is cooled. If the electrons leave the semiconductor from the va lence band, to restore equilibrium some electrons must go over from the conduction band to the valence band, which results in liberation of energy and the crystal being heated. The equilibrium will be main tained and the temperature will remain constant only if the electrons leave the semiconductor from the levels both below and above the Fermi level in appropriate numbers. Theory shows that to maintain equilibrium the average energy of the electrons leaving the semicon
267
Contact Phenomena
ductor should be equal to the Fermi energy, and this is the work func tion although there may be no electrons on the Fermi level itself. The work function is measured in electron volts. The ratio of the work function to the electron charge is the voltage equivalent of the work function. The work function measured in electron volts is nu merically equal to its voltage equivalent. Effect of adsorbed layers on work function. Molecular layers ad sorbed by the surface of the solid, in particular monomolecular layers, greatly affect the work function. Figure 8.3(a) shows a monatomic caesium layer on the surface of tungsten. Caesium is an alkali metal. Its outer valence electron is bonded to the nucleus much more weakly
Figure 8.3 Formation of electric double layer in the course of adsorption of caesium (a) and of oxygen (b) on tungsten surface. , Oxygen ions ( ^
©
©
©
Tungsten ions (b)
than the valence electrons of the tungsten atom. Therefore in the process of adsorption caesium donates its valence electron to tungsten and turns into a positively charged ion inducing a neegative chage of equal magnitude in the m etal’ s surface layer. When tungsten is cov ered by a monatomic caesium layer, an electric double layer is puilt up at the surface with its outer side charged positively. The potential difference in this double layer aids electron emission out of tungsten. Therefore the electron work function, as determined from experiment, drops in the presence of the caesium layer from 4.52 eV for pure tungsten to 1.36 eV. The same is the effect of mon atomic layers of other electropositive metals: barium, cerium, tho rium, etc. The reduction of the work function by the adsorption of electro positive metals is widely used for manufacturing vacuum tube cath odes, photocathodes, etc. Quite different is the effect of oxygen adsorbed on the m etal’ s surface. The valence electrons in the oxygen atom are bonded much
Solid State Physics
268
more strongly than in metals. Therefore in the process of adsorption the oxygen atom instead of donating electrons accepts two electrons from the metal and turns it into a negatively charged ion. As a result the outer side of the electric double layer becomes negatively charged (Figure 8.3(b)) and the resulting electric field prevents the electrons from leaving the metal, thereby increasing the work func tion.
§74 Contact of two metals Contact potential difference. Consider the process which takes place when two metals (Figure 8.4(a)) whose energy diagrams are shown in Figure 8.4(b) are brought together. The electron gas in the individual metals 1 and 2 is characterized by the respective chemical potentials \i±and p2, the thermodynamic Figure 8.4 Origin of contact potential difference betweeiTrctype conductors. 7
d (a)
2
o
work functions being %i and %2 Let us bring the metals closer to gether to within such a distance d that an effective electron exchange by means of thermionic emission or by direct transition from one metal to another is possible. At the initial moment after the contact has been established there will be no equilibrium between the elec tron gas in the first and second metals since the chemical potential (the Fermi level) p,2 is above \i± . The difference in the Fermi levels,
269
Contact Phenomena
p 2 — Pi> results in the prevailing transition of the electrons from the second metal to the first in the course of which the first metal is charged negatively and the second positively. The appearance of the charges causes a shift in the energy levels of the metals: all the levels in the negatively charged metal 1 rise and in the positively charged metal 2 sink as compared with their positions in uncharged metals. This may easily be understood from the following simple consider ations. To move an electron from, for instance, the zero level of an uncharged metal to the zero level of a metal charged negatively to a potential Fx work should be performed numerically equal to q\\. Thiswork is transformed into the potential energy of the elec tron. Therefore the potential energy of an electron occupying the zero level of the negatively charged metal will be higher by the amount qVx than the potential energy of an electron occupying the zero level of the uncharged metal. The zero level of a positively charged metal sinks below the zero level of an uncharged metal the reason for this being the same. A similar shift occurs in the position of other energy levels of the metals 1 and 2 including that of the Fermi level. As soon as the continuously rising chemical potential of the metal 1 (jii) and the continuously sinking chemical potential of the metal 2 (p2) level out (Figure 8.4(c)), the cause for the predominant flow of the electrons from the first metal to the second disappears and a dynamic equilibrium is established between the metals resulting in the corresponding constant potential difference between the zero levels of both metals (Figure 8.4(c)) equal to Pc = (Xi  X.)/? (8.1) This potential difference is termed the external contact potential difference. It follows from (8.1) that it owes its existence to the differ ence in electron work functions of the contacting metals: the elec trons leave the metal with the smaller work function and settle in the metal with the greater work function. After the chemical potentials have been equalized the kinetic ener gy of electrons occupying levels close to the Fermi levels of both met als is not the same: that of electrons in metal 1 is equal to E ¥l and that of electrons in metal 2 to E F2 (EF2 > E Fl). When a direct contact is established between the two metals, a predominant diffu sion process of the electrons from the second metal to the first sets in and continues until the socalled internal contact potential difference
V[ = (EF2 EF[)/q
( 8.2)
is established. Thickness of the electric double layer at the contact of two metals. A double layer (Figure 8.5(a)) is established at the contact of two metals across which the potential changes abruptly by the amount
270
Solid State Physics
V1 (Figure 8.5(b)). Let us estimate the thickness of this layer. Sup pose that it is a plane condenser with the distance between the plates equal to the double layer thickness d. Denote the charge on each plate by Q and the potential difference by Vx. The capacitance of a plane condenser with the plate area of 1 m 2 and a dielectric with relative permittivity e = 1 is C = z jd (e0 is the permittivity of free space). Using the relation C = Q/V{, we can rewrite this formula in the form Q/Vj = e0/d. Hence we obtain d = e0t y Q The thickness of the double layer cannot be less than the lattice parameter a & 3A. At Vi » 1 eV such a layer can be established if Figure 8.5 External (Vc) and internal (Fj) contact potential differences appearing at the instant two different metals are brought in contact.
M (b)
I
a charge Q » V\e0/a « 3 X 10“2 C is transported from every square metre of the contact surface of the first metal to the second. This corresponds to An = Qiq « 2 X 1017 m ~2 electrons. There are ap proximately 1019 atoms on every square metre of a metal. If we as sume that each of them donates to the electron gas one valence elec tron, we will obtain for the surface density of the electron gas the value ns « 1019 m “ 2. Comparing An withrcs, we see that even for the narrowest possible double layer (a « 3A) only two percent of free electrons need be transported from the contact surface of one metal to another. Because of a small change in the electron concentration in the con tact layer and because of the small thickness of this layer in compa rison with the electron mean free path the conductivity of the layer cannot be much less than that of the bulk metal. The current passes through the contact of two metals just as easily as through the metals themselves.
C o n ta c t P h e n o m e n a
27t
§75 The metalsemiconductor contact Barrier layer. Consider a metalsemiconductor contact. Suppose that a metal M with its work function equal to %m is brought in con tact with an ntype semiconductor S whose work function is y* (Figure 8 .6). If Xm > %s> the electrons will flow out of the semiconductor into the metal until the chemical potentials pm and jns are equalized and a state of equilibrium is established. A contact potential difference Fc will be established between the metal and the semiconductor whose order of magnitude will be the same as that in the metalmetal contact (several volts). To establish such a contact potential F ig u re 8.6
Formation of barrier layer in metalsemiconductor contact.
difference approximately the same number of electrons should be transported from the semiconductor to the metal as in the case of the contact of two metals. For a lattice parameter of the semiconduc tor A (germanium) and an electron gas concentration in it n & 1021 m ~3 there will be ns & 1014 electrons on 1 m 2 of the semi conductor’ s surface. Therefore the transport of An « 1017 electrons entails the “ depletion”of about 103 atomic layers of the semiconduc tor. Hence the equalization of the chemical potentials of a metal and a semiconductor in contact with one another necessarily involves the transport of electrons to the metal surface from a boundary layer of appreciable width d of the semiconductor (Figure 8 .6). The ionized impurity atoms remaining in this layer establish a static positive space charge. Since there are practically no free charge carriers inside this layer and since its width greatly exceeds the electron mean free path, its specific resistance is very great and be cause of that it is termed barrier layer. Effect of contact field on semiconductor energy levels. The contact potential difference Vc between the metal and the semiconductor is built up over the entire width d of the barrier layer (Figure 8 .6). Assuming that 5 A,we obtain for the number of depleted atomic layers AAr ^ 103 and for the thickness of the barrier layer d ^ « 5 X 103 A « 5 X 10" 7 m. For Vc « 1 V the field intensity will be g c « VJd « 2 X 106 V/m. This is at least three orders of mag
1272
Solid State Physics
nitude less than the intensity of the internal crystal field, which is responsible for the energy band pattern of the semiconductor. There fore the contact field cannot appreciably affect the band spectrum (the forbidden band width, the impurity ionization energy, etc.). Its action is limited to the deflection of the semiconductor’ s energy bands. Let us dwell on this. Figure 8.7(a) shows the energy band diagrams of the metal M and the semiconductor S before they have been brought in contact. When F ig u r e 8.7 Effect of contact field on semiconductor’ s energy levels: {a)—band patterns of metal M and semiconductor S\ (b)—deflection of semiconductor’ s energy bands by contact field.
contact has been achieved and equilibrium has been established, a positive space charge throughout the barrier layer width d is built up (Figure 8.7(b)). In the absence of the contact field the energy levels in the metal and in the semiconductor are represented by horizontal straight lines. This expresses the fact that the energy of an electron occupying this level, for instance, the lower level of the conduction band, is the same everywhere in the semiconductor and does not depend on the position of the electrons. In the presence of a contact potential difference the picture is changed: inside the layer in which the contact field is concentrated a force acts on the electron pushing it out of the layer. To overcome this force work should be performed, this work being equal to the potential energy of the electron in the contact field. Therefore as the electron moves inside the space charge layer its potential energy cp (x) increases reaching its maximum cp0 =
273
Contact Phenomena
= qVc at the semiconductor’ s surface. Quantum mechanical calcu lations lead to the conclusion that the application of an external field to the semiconductor results in an inclination of its energy bands in relation to the horizontal Fermi level. The contact field acts in the same way causing a deflection of the energy bands. The quantity cp0 is termed the equilibrium potential barrier for electrons going over from the semiconductor to the metal. To estimate the function (x) we apply the Poisson equation known from electrostatics. This equation relates the field potential V (x) to the density p (x) of the static space charge responsible for this field. The equation is of the form d2V dx2
p
(x)
e 0e
(8.3)
where e is the relative permittivity of the semiconductor. It is expedient to go over from the potential V (#) to the potential energy of the electron cp (x) = — qV (x) and to write the Poisson equation for
p
h2
T
^3/2 /1_ E J ( 2 k u T ) 6
/
It may easily be seen that nYwill rise rapidly with the increase in temperature while nn0 « iVd and p p0 « A awill remain practically constant. Therefore at some temperature n{ may become as high as nn0 or pp0. Then the concentrations of the minority carriers will be as high as the concentrations of the majority carriers: Pno = n\/nno « n l0/nn0 = nn0 and np0 = n\/pp0 « p 2 Po/pPo = P po . The potential barrier in the pn junction which is responsible for
Contact Phenomena
287
its rectifying properties will then cease to exist: d will be reached at which the resistance of the barrier layer drops drastically and the reverse current jumps up. This phenomenon became known as the pn junction breakdown (Figure 8.16). There are different types of breakdown: thermal, tunnel (or Zener), and the avalanche breakdown in accordance with the nature of the physical processes that cause the reverse current to grow abruptly. Thermal breakdown occurs when the heat generated by the reverse current flowing through the pn junction is not completely removed from it and raises its temperature. A rising temperature leads to an increase in the reverse current and this, in its turn, raises the temper ature still further, etc. This progressive process results eventually in thermal breakdown. The character of the increase in current during such a breakdown is depicted in Figure 8.16, curve 1. When the electric field intensity in the pn junction is high enough, impact ionization of the atoms of the semiconductor may take place. This will result in an avalanchetype increase in the carrier con centration and in the avalanche breakdown; the character of the increase in current is shown in Figure 8.16, curve 2. In a narrow pn junction already at comparatively low reverse voltages an electric field may be established high enough for the tunnelling of the electrons through the pn barrier to take place. The resulting breakdown is termed tunnel, or Zener, breakdown
288
Solid State Physics
and the character of current increase iT (V) for this case is shown in Figure 8.16, curve 3. In most cases the pn junction breakdown is a harmful effect that limits the practical use of the junction. At the same time the effect was utilized to develop a wide range of semiconductor devices known as Zener diode voltage regulators, which will be discussed in the following section.
§77 Physical principles of semiconductor p  n junction devices As had already been stated before, the rapid progress in semiconduc tor electronics was the direct result of the development of the pn junction technology on which the design of various semiconductor devices is based. Let us discuss the general principles of such devices. Figure 8.17 Schematic representation of a rectifier diode: 1—pn junction, 2 and 3—passive regions, 4—ohmic contacts.
Rectifier diodes. The nonlinear currentvoltage characteristic of the pn junction (Figure 8.15) enables it to be used to rectify alter nating current. A twoterminal semiconductor device fulfilling such function is termed semiconductor rectifier diode. Figure 8.17 shows the principal schematic diagram of such a diode. It consists of a pn junction i, passive n and pregions 2 and 5, and ohmic contacts 4. The highresistivity region of the crystal is termed base of the diode. In our case it is the ^region 3 of the width W. Nowadays pn junction rectifier diodes are made almost exclusive ly of silicon. The efficiency of such diodes is almost 100 percent and in combination with their low weight, small dimensions, ease of servicing, etc. this made them a very widely used device for such applications. Various diode types are designed to rectify currents from several milliamperes to several hundred or thousand amperes. For greater currents the diodes are connected in parallel. The maxi mum reverse voltage for various types lies in the range from 50 to 600 V. It may be much higher for special diode types. For use in highvoltage rectifiers the diodes are assembled inseries in stacks. The reverse currents of various rectifier types lie in the range from fractions of a microampere to tens of milliamperes.
Contact Phenomena
289
Impulse and highfrequency diodes. The second very important field of application of the semiconductor diodes is the field of impulse electronics, computer electronics, automation, VHF electronics, etc. In such applications the diode is required to process pulses of mini mum duration and of maximum repetition rate. Therefore one of the main requirements of diodes designed for such circuits is the speed of operation, that is, switching speed from the direct to the reverse F ig u r e 8.18 T ran sien t p rocesses in diode: (a)— m a jo rity and m in o rity carrier distrib u tion s; (b)— m in o rity carrier in jection b y forw ard v olta ge and their diffusion in to the b u lk o f sem icon d u ctor; (c, d)— v ariation s o f forw ard and reverse v olta ge s and curren ts in a d io d e sw itch ed on in the forw ard direction and resw itch ed to reverse direction .
state. To find what lies at the origin of this speed let us discuss the physical processes that take place when a pn junction is switched. Figure 8.18(a) shows the distribution of the majority and minority carriers in the p  and nregions of an equilibrium pn junction. When a direct voltage V is applied to the diode, the potential barrier of its pn junction sinks by qV and the majority carrier flux through the junction increases e^v/hBT times with the result that the hole concentration at boundary 1 and the electron concentration at boun dary 2 rise to the values of pn (0) pn0 and np (0) np0J respec tively (Figure 8.18(b)). For the direct current to flow it is necessary for those carriers to be drawn into the bulk of the semiconductor: the holes should be drawn into the raregion and the electrons into the pregion. The recombination of those minority carriers takes place inside the regions, or on the contacts if the width of the regions is small in comparison with their diffusion length. The removal of the minority carriers proceeds either by means of diffusion whose rate is the higher the greater the concentration gradient of holes
290
S o l id S ta te P h y sics
(idp/dx) at boundary 2 and that of electrons ( R [n), a v 1 and may be as high as 105 (for dc current). Since in this connection only the voltage is amplified, the same will be the power amplification factor a P = Pout^m « » a v. The source of the additional signal power dissipated in the collector circuit is the collector power supply Fc. Figure 8.22(b) shows the transistor connected into a common emit ter circuit. In this case the signal from the source S is applied between the emitter and the base, the output signal being taken off the emitter and the collector. The input signal affects the emitter /e, the collector 7C, and the base /b currents, the latter being the difference of the former two (/b = I e — /c). Since /c = a /e, it follows that the common emitter current amplification factor R= ^°_ a p 7b 7e/c l a can be made very high ( ~ 104), but from considerations of stability and of frequency response it is usually held in modern transistors in the range from 40 to 100. Transistors have found universal application in electronics: in low and highfrequency amplifier and oscillator circuits, in
Contact Phenomena
295
switching circuits, in triggers and multivibrators, in low and highfrequency detector circuits, etc. Almost the whole of modern com mercial and specialpurpose electronics is based on semiconductor devices the most important of which is the transistor. Photoelectric devices; p  n junction photocells. When a pn junction is illuminated an emf is established in it. This phenomenon is uti lized in barrier layer photocells which may serve as indicators of Figure 8.23 Semiconductor barrier layer photocell: (a)—schematic representation; (b)—energy band pattern of pn junction.
radiative energy independent of external power sources and as con verters of radiative energy into electrical energy. Figure 8.23(a) shows the schematic representation of a photocell. A narrow diffused zzlayer is fabricated on the surface of a ptype semiconductor wafer so that a pn junction is formed. In the absence of illumination the pn junction is in the state of equilibrium and an equilibrium potential barrier qVc (Figure 8.23(b)) is established in it. When the junction is illuminated, electronhole pairs are generated mostly in the pregion because light passes through the narrow zzlayer without absorption. The electrons generated in the pregion diffuse to the pn junction and are drawn in by the contact field and transported to the zzregion. The holes are unable to sur mount the barrier qVc and remain in the pregion. Because of that the pregion acquires a positive charge and the zzregion a negative one and an additional forward voltage FPh is established across the junction. The term for it is photoemf, or photovoltage. At present the most efficient converters of solar energy are silicon photocells (solar batteries). They are used as power supplies for receivers and transmitters installed on satellites and even on the
296
Solid State Physics
ground. Calculations show the maximum efficiency (theoretical) of the silicon energy converters to be as high as 2223 percent. The* efficiency of the best modern types is about 15 percent. Germanium, copper oxide, selenium, silver sulfide, sulfurous thallium and other semiconductor photodiodes are widely used as indicators of radiative energy. Their integral (in the entire spectrum) sensitivity is much higher (102103 times) than that of the external photoeffect cells. Their main disadvantage is their great inertiality. Photodiodes. The photodiode is a photocell connected into a circuit inseries with an external power supply (Figure 8.24(a)). In the Figure 8.24 Photodiode: circuit diagram (a) and currentvoltage characteristic (b).
yr V°
2
'M
0
________
j
'*r (b) absence of illumination I a negligible socalled dark current flows through the junction (Figure 8.24(b)). When the pn junction is illuminated, excess carriers are generated and the current rises in proportion to I causing a voltage drop across the load resistor R\. Substantial advantages of the photodiodes over the external photoef fect elements are smaller dimensions and lower weight, high integral sensitivity and low operating voltage. Luminescent dipdes. The passage of a forward current through the pn junction involves, as we know, minority carrier injection: of electrons into the pregion and of holes into the ^region. The injected carriers recombine with the majority carriers of the respec tive region, their intensity decreasing with the distance from the pn junction (Figure 8.18(b)). In many semiconductors the recom bination is nonradiative: the energy liberated in the recombination process is absorbed by the crystal lattice, that is, turns eventually into heat. However, in such semiconductors as SiC, GaAs, InAs, GaP, and InSb the recombination is radiative: the energy of recom bination is liberated in the form of radiation quanta, photons.
29 7
C on ta ct P h en om en a
Because of that a forward current flowing through the pn junction made of such materials is accompanied by the emission of light from the junction region. This phenomenon is utilized in the luminescent diodes. Such diodes are used in displays, they may be used in computers for data input and output and in other applications requiring reliable lumi nous indicators. Low operating voltages, low power consumption and a long service life are the advantages of the light emission diodesover other electroluminescent light sources. Semiconductor lasers. In recent years intensive work has been in progress on the semiconductor sources of coherent radiation—semi conductor lasers—which open up possibilities for the direct conver sion of electric energy into the energy of coherent radiation. In Figure 8.25(a) the solid line shows the electron distribution corresponding to the equilibrium state and the dotted line the distri bution corresponding to the nonequilibrium state, in which theconcentrations of electrons in the conduction band and of the holes in the valence band are above the equilibrium values. Such band occupancy corresponding to population inversion is shown in Fig ure 8.25(b). The peculiar point about it is that the light quanta with the energy Hco = E g (Eg is the forbidden band width) cannot beabsorbed by the system. Indeed, such an absorption involves the transfer of an electron from the top level of the valence band to the lowest level of the conduction band. Since there are practically no electrons on the top levels of the valence band and no vacant states at the bottom of the conduction band the probability of such a process is extremely small. This creates favourable conditions for the stimulated emission and for an avalanche of photons. Tim light quantum 1 (Figure 8.25(b)) stimulates the recombination o f the electron and the hole (atransition), which results in the emis sion of an identical quantum 2. Since the quanta are not absorbed; Figure 8.25 (a)—electron distribution plots for equilibrium (solid line) and inverse (dotted line) states of semiconductor; (b)—development of photon avalanche caused by induced radiation of a quantum system with population inversion; (c)—in a quantum generator only the radiation which propagates along the 00' axis is amplified.
(a)
(b)
(c)
Solid State Physics
298
by the system, they subsequently stimulate the emission of two new quanta, etc. To make one photon take part in many stimulated emission acts, two strictly parallel mirrors 1 and 2 (Figure 8.25(c)) are arranged on the opposite sides of the laser crystal to reflect the incident photons and return them into the crystal. Only those pho tons are amplified which move strictly along the 00' axis, for only such photons are repeatedly reflected by mirrors 1 and 2. All other photons leave the active laser space immediately or after a limited number of reflections (in Figure 8.25(c) such photons are shown by
w
Figure 8.26 Schematic representation of semiconductor laser: 1— active region of laser; 2— reflecting faces (mirrors)
dotted lines). The result is a highly directional and highly monochro matic beam of radiation along the 00' axis. There are various methods of creating a population inversion of the semiconductor energy bands. The best prospects offers the minority carrier injection through a forward biased pn junction made in a degenerate semiconductor. Figure 8.26 shows the structure of a semiconductor laser in which such method of pumping is used. The laser is a diode with a pn junction 1 made in the form of a bar. Highly polished faces 2 of this bar made strictly parallel to each other play the part • of mirrors that reflect the photons. The interest for the semiconductor lasers is due to some of their remarkable properties. First of all, they have a high efficiency which may in principle reach 100 percent. This is due, on the one hand, to the quantum mechanical nature of the laser as a system in which only the “ working” energy levels are excited, and on the other, to the fact that in a semi conductor laser the electric energy is directly converted into coherent radiation without any intermediate steps as in all the other laser types. Another remarkable property of the semiconductor laser is that it is possible to modulate the coherent radiation directly by changing the current through the pn junction. This enables them to be used in communications and in television as well as in ultrahighspeed computers for which their miniature dimensions are of special impor tance.
Contact Phenomena
299
§78 Fundamentals of integrated circuit electronics (microelectronics) The progress of modern science and technology requires electronics to provide for it efficient complex electronic equipment. Such equip ment often contains hundreds of thousands of elements connected into a circuit by means of a similar number of connections. Electronic equipment is responsible for the main part of costs of production of modern military equipment and aircraft. Accord ing to Western sources, the cost of electronic equipment makes up over 70 percent of the cost of a modern guided missile and over 50 percent of the cost of a modern bomber. To produce such highly sophisticated equipment some difficult problems had to be solved, including the problems of drastic reduc tion in weight, dimensions, power consumption, and in price and of increasing the reliability of electronic devices. Should modern electronic apparatus be assembled from compo nents manufactured by the industry several decades ago, its weight would have been tons, its dimensions cubic metres, and its power consumption hundreds of kilowatts. The latter fact would have sufficed to make it impractical for many fields of the economy. But those are not the only drawbacks. As the complexity of the electronic equipment increases its reliability—a factor of primary importance especially in military, computer and automatic produc tion line applications—diminishes. Finally, the problem of bringing down the costs of electronic equipment is also not devoid of importance and this problem can only be solved by farreaching automation of the technological processes, which in turn requires the development of appropriate technology. The efforts to solve those problems lead to the creation of minia ture electronic elements and blocks based on solidstate technology and to the microminiaturization of electronic equipment resulting finally in the birth of a new field of modern electronics—microelec tronics—whose main objective is the production of highly reliable and economical microminiature electronic circuits and apparatus. The modern way to solve this problem is to devise new principles of constructing electronic circuitry which would make possible the formation of a circuit as a whole on a miniature semiconductor crystal instead of assembling it from separate components. Such solid electronic circuits designed for specific applications are termed integrated circuits (IC). The integrated circuit, like an ordinary electronic circuit, is made up of active elements (transistors, diodes) and of passive elements (capacitors and resistors).
300
Solid State Physics
A semiconductor IC is fabricated on a singlecrystal wafer (usually silicon) with the aid of methods of local doping with appropriate impurities to produce on it transistors, diodes, capacitors, and resistors and to connect them into a circuit. The dimensions of the wafer are typically (10~2) X (5 X 10~3) X (2 X 10“ 4) m3, the area of the active elements, for instance of a transistor, being under
10~9 m2. The integrated circuits are usually characterized by packing density and by degree of integration. The packing density is the number of elements per unit volume of the IG, and the degree of integration, the number of elements making up the IC. Table 8.2 presents data on the packing density and on failure rate of circuits of different generations. Table 8.2
Circuits using Pre1941 elements Miniature elements Semiconductor IC
3.5 X 1 0 4 1.8x105 3.0x10®
105 5X1(T6
Negligible
It follows then that the changeover from the circuits assembled from pre1941 components to modern IC increased the packing density some 105 times. There are reports of packing densities of IC of up to 1015 m “ 3. The degree of integration of an IC may vary in a wide range— from tens to hundreds or thousands of elements on each wafer. IC of over 100 elements are termed big integrated circuits (BIC). The power consumption of IC, depending on the type, lies in the range of hundreds of milliwatts to several microwatts. Thus, the changeover to electronic equipment designed around IC practically solved the problems of dimensions, weight, and power consumption. Electronic computers are an impressive example of this. The first Soviet computers which were assembled from vacuum tubes and radio components (Minsk, Ural, etc.) occupied whole buildings, weighed tons, and cosumed tens of kilowatts of power. Electronic blocks assembled from IC have dimensions of the order of 10“2 m3 and consume only hundreds of watts while special comput ers used, for instance, for launching and controlling missiles and spacecraft have dimensions of the order of 10“3 m3, weigh tens of kilograms and consume power of the order of tens of watts. Presently BIC are being used in single wafer electronic calculators. The computer wafer (called “ chip” ) of such a device is (5 X 5)10“6 m 2 and contains about 5 thousand transistors. BIC for electronic time
Contact Phenomena
301
pieces including wrist watches have been developed as well. In such watches two wafers containing about 2 thousand transistors are used. A substantial advantage of IG is that because massproduced IC are much cheaper than equivalent circuits assembled from compo nents. Modern technology makes it possible to arrange about a thou sand IG on one singlecrystal wafer of 5 X 10" 2 m in diameter; if a hundred such wafers are processed at a time, about a million IC can be produced in one technological cycle. The progress in microelectronics is a very rapid one. During the last decade a distance was covered from the simplest IC to BIC. In the nearest future it is expected that most electronic equipment shall be based on integrated circuitry with the degree of integration increasing 100 to 1000fold and a much greater reliability being attained. However, there are obstacles on this road, namely the socalled “ tyranny of numbers” of microelements which already today crowd complex equipment in tens or hundreds of millions. To overcome this obstacle it will, probably, be necessary to change over from the conventional IC to functional circuits, that is, to devices designed for specific functions and operating on some specific prin ciple of solid state physics as a whole and not as a sum of individual elements (transistors, diodes, etc.). As the simplest example of a functional device one may cite the acdc converter. The conventional circuit of such a converter consists of a transformer, rectifiers (semiconductor or vacuum diodes), and a filter. The functional converter consists of a resistance region in which the ac energy is transformed into heat, of the central low electric but high heat conductivity region, and of a thermoelectric region in which heat is converted into dc power. In such a device it is impossible to separate regions equivalent to the components of a conventional circuit. Here the crystal as a whole fulfills the complex function of an acdc converter. The transition to functional circuits should result in a drastic decrease in the number of components and therefore in the decrease in the cost and in dimensions and in the improvement of reliability. The process of creation of new scientific and technological trends in electronics and of devising devices and equipment based on new principles is a continuous one, the foundation for it being the utili zation of the topranking achievements in the fundamental and applied sciences, first of all, in physics. Here the leading role belongs to solid state physics which determines the mainstream of progress in modern electronics.
9 Thermoelectric and Galvanomagnetic Phenomena
The thermoelectric effects include the Seebeck, the Peltier, and the Thomson effects, and the galvanomagnetic the Hall, the Ettingshausen, and the Nernst effects. Some of those phenomena have found wide application in practice; therefore a look at them is not only of educational but of practical interest as well. Let us discuss briefly the physical background of those phenomena.
§79 The Seebeck effect In 1822 T. J. Seebeck discovered that an electromotive force VT is established in a circuit consisting of two conductors 1 and 2 made of different materials if the junctions of these conductors, A and B y are kept at different temperatures, Tx and T2 (Figure 9.1(a)). This emf is termed thermal emf. Experiments show it to be—in a narrow temperature interval—proportional to the difference in the tem perature of the junctions A and B: VT = a (T2  Tx)
(9.1)
The proportionality factor a = dVt ldT
(9.2)
is called differential, or specific, thermoelectric power. It is deter mined by the material of the conductors and the temperature. There are three sources of thermal emf: the directional current of the carriers in the conductor due to the presence of a temperature gradient (the volumetric component V\), the change in the position of the Fermi level (the junction component V]), and the drag of the electrons by the phonons (the socalled phonon drag effect). Let us discuss the physical nature of each of those sources. Volumetric component of thermal emf. Suppose that a temperature difference (T2 — Tx) is maintained at the terminals of a uniform conductor AB (Figure 9.1(b)) so that there is a temperature gradient 302
303
Thermoelectric and Galvanomagnetic Phenomena
dT/dx in the direction from B to A . The current carriers in the hot end have greater kinetic energy and greater speeds of motion than the carriers in the cold end. Therefore a current will flow in the conductor from the hot end to the cold; this current will charge the conductor. In cases when the current is carried by electrons, the cold end will accumulate a negative charge and the hot end a posi tive charge, and a potential difference Fv will be established between Figure 9.1 The Seebeck effect: (a)—thermoelectric circuit; (b)—origin of volumetric and junction components of thermal emf.
them. This is the volumetric component of thermal emf. The differen tial thermoelectric power corresponding to this component is (9 3 >
a v may be estimated as follows. The pressure of the electron gas in the conductor is p = ~nE (9.4) where E is the average energy of electrons in the conductor, and n their concentration. The temperature gradient occasions a pressure gradient to com pensate which a field % should be established in the conductor such that dp dx
dp
dT
dT
dx
From here a v may easily be found: dVy
c£ / dT \  i
aV— 5 f= *(te)
1
dp
/n Kv
As a rule, in an ntype conductor a v is directed from the hot end to the cold. However, there are exceptions to this rule which we will discuss below.
304
Solid State Physics
The junction component of thermal emf. The change in temperature occasions a change in the position of the Fermi level. In rctype conductors the Fermi level sinks on the energy diagram as the temper ature is raised (see Figure 5.19(a)). By force of this it should be higher on the cold end of an ratype conductor than on its hot end. The difference in the Fermi level positions is equivalent to a poten tial difference dv> =  \ w dT
(96)
And this is just the junction component of the thermal emf. The dif ferential thermoelectric power corresponding to this component is a = __ I dpi (9.7) It The resultant differential thermoelectric power 1 dp nq dT
1 djit q dT
(9.8)
We apply the relation (9.8) to conductors of various kinds. Thermoelectric power of metals. Substituting the average energy o f electrons of a degenerate electron gas from (3.45) into (9.4), we obtain the following expression for the pressure of the electron gas in a metal: p  t " b = t ”£' + w ( w differentiating this expression with respect to T and multiplying it by ilnq, we obtain __/cB ji2 kBT av~ q 3 E¥
(9.9)
The temperature dependence of the Fermi level in metals is given by relation (3.44):
Differentiating it with respect to T and multiplying by 1!q% we obtain 3T2A;b k^T (9.10) 6q
Ey
Substituting (9.9) and (9.10) into (9.8), we obtain
a" “T r ( 1 + 4  )  i r
(9,1)
A more accurate calculation for metals with a quadratic depen dence of the electron energy on the wave vector produces the fol
Thermoelectric and Galvanomagnetic Phenomena
305
lowing result: (9.12)
o .  ^ d + r ) # where r is the exponent in the relation roc
, (9.13)
et
which expresses the dependence of the electron mean free path on energy E. % Table 9.1 presents the values of r for various mechanisms of elec tron scattering on atomicand ionic lattices. Table 9.1 Scattering on thermal vibrations Ionic lattice
Atomic lattice r
A ~
0
re 1
Scattering on impurity atoms 2
It follows from (9.12) that for metals a m a T, in full agreement with experiment. Since kB T E F the thermoelectric power of metals is quite small. For instance, for silver E F = 5.5 eV and kB T = 0.025 eV at T — 300 K; substituting this into (9.12) we obtain a m « 8 X 10~6.V/K, which is quite close to the experimen tal value a m » 5 X 10~6 V/K. It follows from (9.13) that when r < 0 the more energetic elec trons have a shorter mean free path X. Since the diffusion current in this case is directed from the hot end to the cold end, the sign of the volumetric component of the thermal emf will be reversed. This may cause the reversal of the sign of the m etal’ s thermal emf as a whole. Such effects are observed, for example, in some transition metals and in some alloys. As was already stated before formula (9.12) is valid for metals with a quadratic E (k) dependence. In metals and in alloys with a complex Fermi surface the contribution of the various regions of this surface may differ not only in absolute value but in sign as well, with the result that the thermoelectric power may be zero or close to zero. For instance, lead has a zero thermoelectric power. For this reason thermoelectric power is usually measured in relation to lead. ~ . The current direction in the hot junction of a thermocouple made of an ratype conductor and of lead will be determined by the polarity of the conductor’ s charge. For a normal conductor whose hot junction acquires a positive charge the current in it will be directed from 200885
Solid State Physics
306
conductor to lead (Figure 9.2(a)). In this case the conductor’ s ther moelectric power is assumed to be negative. In case of an ratype conductor acquiring an anomalous charge* (Figure 9.2(b)) the current in the hot junction will flow from lead to conductor and a will be positive; X will be positive for a normal
a
ntype conductor +
Pb
I
Hot junction
Figure 9.2 Magnitude and sign of thermoelectric power determined in relation to lead (explanation in text).
ype con due to r Pb
TflHot junction
7 bT
p type conductor
Pb
/
Hot junction
(c)
jotype conductor too, whose hot end acquires a negative charge (Figure 9.2(c)). Thermoelectric power of semiconductors. The pressure of electron gas in a nondegenerate semiconductor is p=
nE = nkBT
Differentiating this expression with respect to T and multiplying by l/nq, we obtain (9.14) Oy —— [ i + r ^ ] A more rigorous calculation yields a c= kB r> 1 1 , rp d\nn (9.15) V Q l r + 2 + T dT ■] The chemical potential in a nondegenerate ntype semiconductor is given by relation (3.26): Kn — k B T In
2 (2nmnk BT)3/3
Differentiating pn with respect to T and multiplying by ilq , we obtain r)
Substituting (9.15) and (9.16) into (9.8), we obtain an
Q
(r + 2
M'n \ _ kBT ) ~
I"  o  l — ^ (2nmnkBT)3/2 q [ + “+ n nh3
(9.17)
Thermoelectric and Calvanomagnetic Phenomena
307
The minus sign in front of the righthand side jis in accordance with the conventional polarity of the thermoelectric power. For a rctype semiconductor + 2+
(9.18,
Let us estimate the value of a of an extrinsic semiconductor, for instance, for rctype germanium with n = 1023 m ~3 at T = 300 K. Substituting those values into (9.17), we obtain a « 10" 3 V/K. Hence the thermoelectric power of semiconductors is three orders of magnitude greater than that of metals. For semiconductors with bipolar conductivity, in which the electric current is carried both by electrons and holes, the expression for the thermoelectric power is: a n,p
&pPup — &nnun pup + nun
(9.19)
It follows from this relation that if the electron and hole concentra tions and their mobilities turn out to be equal, the thermoelectric power may be quite small or even zero. Phonon drag of electrons. The phonon drag effect, discovered by L. E. Gurevich in 1945, consists in the following. With a temperature gradient in the conductor the phonons drift from its hot end to the cold end at an average velocity i;Ph. In the presence of such drift the electrons scattered by the drifting phonons are themselves in volved in the directional motion from the hot end to the cold end, their velocity being about equal to z;Ph. The accumulation of the electrons on the cold end of the conductor and their depletion on the hot end results in the appearance of a thermal emf FPh. G. E. Pikus in 1956 calculated the differential thermoelectric power due to the phonon drag and obtained the following result: aph
Arp mnvph Tph *3?
(9.20)
Here i?Ph is the phonon drift velocity,, and Tph and x e are the phonon and electron relaxation times. In the low temperature range this component of thermoelectric power can be tens or hundreds of times greater than the volumetric and junction components.
§80 The Peltier effect Let a current I flow in a circuit consisting of two conductors 1 and 2 (Figure 9.3) made of different materials. The Joule heat Q = = P R t will be liberated in the junctions A and B (R is the junc20*
308
Solid State Physics
tion ’ s resistance, and t is the time the current flows). At junctions of identical conductors only this heat will be liberated and from this point of view there is no difference between the junction and the* rest of the circuit. At the same time at points of junction of different materials an additional heat apart from the Joule heat will be liber ated or absorbed, heating the contact in the former case or cooling it in the latter. This phenomenon was discovered in 1834 by Figure 9.3 Diagram of circuit used to observe the Peltier effect.
J. C. A. Peltier and is termed the Peltier effect; the additional heat liberated or absorbed in the junction is termed Peltier heat, Qp. Experiments show it to be proportional to the current I and the time the current passes through the contact t: QP = n It
(9.21)
The proportionality factor II is termed the Peltier coefficient. Its value is determined by the materials and by temperature. There is a direct connection between the Peltier and Seebeck effects: the temperature difference causes a current to flow in a cir cuit consisting of different materials and a current flowing through such a circuit sets up a temperature difference. The expression for this relation is due to W. Thomson (Lord Kelvin), who is the author of the thermodynamic theory of thermoelectric phenomena. He demonstrated that: a = U/T
(9.22)
The Peltier effect is due to the difference in the average energies of the conduction electrons in unlike materials. By way of an exam ple, let’ s consider the junction of a metal with a nondegenerate ratype semiconductor (Figure 9.4). After equilibrium had been estab lished their Fermi levels will coincide. Only the electrons close to the Fermi level whose average energy are practically equal to the Fermi energy take part in the conductivity in the metal. Denote the average energy of the conduction electrons in the semiconductor by E n. This energy is not equal to the thermal energy of the electrons 3kBT/2 since the relative part played by fast elec trons in the electric current is greater than that of slow electrons. A calculation made for the case of a nondegenerate electron gas
Thermoelectric and Calvanomagnetic Phenomena
309
yields E n = (r + 2)kBT
(9.23)
where r is the exponent in (9.13). Suppose that the electric current flowing through the junction is such that the electrons flow from the semiconductor to the metal. Metal
ntype semiconductor
Figure 9.4 Energy band pattern of metalsemiconductor junction illustrating mechanism of the Peltier effect.
It may be seen from Figure 9.4 that each electron that goes over from the semiconductor to the metal carries with it an additional energy equal to AE = E n + (  i i n)
(9.24)
This energy is the Peltier heat and it is liberated near the junction. When the direction of the current is changed, the electrons going over from the metal to the semiconductor absorb heat and cool the junction. Dividing AE by the electron charge, we obtain the Peltier coef ficient: n mn —
AE
(9.25)
 ( £ n ~ * 0
Substituting u from (3.26) and E n from (9.23) into (9.25), we obtain n mn =
—
[ (r + 2) + In 2
W
/2 ]
(9.26)
A similar relation may be obtained for the junction of a metal with a ptype semiconductor n mp *
[ (r + 2)+ln
2 (2nmpkftT)3/2
ph*
(9.27)
310
Solid State Physics
For a junction of two metals the Peltier coefficient may be found from (9.22): IIi,2= (a4— a 2) T (9.28) Substituting a from (9.12), we obtain Hi,2
n2k2BT2
3q
0
Scattering by im purity ions
1.17
0.99
1.93
1.11
of this, other conditions equal, their Hall emf and Hall coefficients will be smaller than in unipolar semiconductors. Calculation yields the following expression for i?H of bipolar semiconductors: A upp —unn q (upp + u nn)2
(9.38)
where n and p are electron and hole concentrations, and un and up their mobilities. Depending on which of the two terms in the nu merator is greater, the sign of the Hall coefficient may either be posi tive, or negative. For intrinsic semiconductors, in which n — rii formula (9.38)> assumes the form: A UP u n n\q «p+«n
(9.39)
It follows from (9.39) that in the intrinsic range the sign of the Hall coefficient is determined by that of the carriers with greater m obili ty. As a rule such carriers are electrons. Therefore when an extrin sic jotype semiconductor goes over to the intrinsic range, the sign of the Hall coefficients changes. Hall coefficient (at room tempera ture) for some metals and intrinsic semiconductors is presented below in Table 9.3. Table 9.3
i?H (10"11 m3/C)
Cu
Zn
Bi
Ge
Si
5.5
3.3
103
1010
1013
As indicated, the Hall coefficient of semiconductors is many orders of magnitude greater than that of metals. The explanation is that the carrier concentration in semiconductors is much less but the mobility, on the other hand, is much greater than in metals. Ettingshausen effect. The thermal velocities of electrons in non degenerate semiconductors lie in a wide range. In such conditions equation (9.33) may be valid not for all the electrons but only for some of them whose average velocity is v0. For electrons whose
314
Solid State Physics
■velocity is v > v0 we have quB > q(SH and they will be deflected to the righthand face of the plate (Figure 9.6(a)). The electrons whose velocity is u < v0y so that qvB
Comparing (1.7) with (1.8), we obtain 1
df(Ex)
1
d/(ff2)
(1.9) / (^1) / (^2) ^ ^ 2 The lefthand side of (1.9) is independent of E 2, the righthand side is independent of E x; therefore each of them is equal to some constant independent of the particles’energy. Denote it by p. Then we may rewrite (1.9) as follows:
1 / {E)
if(E) dE
q P
(i.io>
Integrating (1.10), we obtain / (E) = Ae$E
(I.ll)
where A is the integration constant. Experiment shows that p = — (kBT)\
A = e'l/hbt
(1.12)
Substituting (1.12) into (I.ll), we obtain U E ) = e ^ eElk^
(1.13)
Appendix II Derivation of the FermiDirac distribution function. Consider, as we did in Appendix I, the direct and reverse particle collisions. Recall that in the case of a nondegenerate gas the rate of collisions was independent of the number of particles in the final stages and was entirely determined by the number of particles in the initial stages. The situation in the case of a degenerate fermion gas is a different one: if a state is already occupied, it cannot accept another fermion and the collision will not take place. For this reason in the case of a degenerate fermion gas the rate of collisions is proportional not only to the average number of particles in the initial states but
Appendix II
319»
to the average number of vacant states with the energies E 3 and as well. Since /F (E) expresses the probability for the state with the ener gy E to be occupied, 1 — /F (E ) expresses the probability for it to be vacant. Therefore the average numbers of vacant states with the energies E 3 and E k are 1 — /F (E3) and 1 — /F (£4), respective ly. Accordingly, the rates of direct and reverse collisions are: